Upload
others
View
15
Download
0
Embed Size (px)
Citation preview
i
FABRICATION AND CHARACTERIZATION OF NOVEL
TRANSPARENT LAMINATED GLASSCOMPOSITE
PANELS FOR DYNAMIC LOAD MITIGATION
_______________________________________________________
A Dissertation
Presented to
the Faculty of the Graduate School
University of Missouri
_______________________________________________________
In Partial Fulfillment
of the Requirements for the Degree
Doctor of Philosophy
_______________________________________________________
by
HUA ZHU
Dr. Sanjeev K. Khanna, Dissertation Supervisor
MAY 2014
The undersigned, appointed by the dean of the Graduate School, have examined the
dissertation entitled
FABRICATION AND CHARACTERIZATION OF NOVEL
TRANSPARENT LAMINATED GLASSCOMPOSITE PANELS FOR
DYNAMIC LOAD MITIGATION
presented by Hua Zhu,
a candidate for the degree of Doctor of Philosophy,
and hereby certify that, in their opinion, it is worthy of acceptance.
Professor Sanjeev K. Khanna
Professor Robert A. Winholtz
Professor Qingsong Yu
Professor Raghuraman Kannan
Dedication
This dissertation is dedicated to my beloved mother
Shan Wang (19532008)
You are profoundly appreciated for your
support of my academic pursuits.
ii
ACKNOWLEDGEMENTS
I would like to take this opportunity to express my sincere gratitude to my advisor
Dr. Sanjeev K. Khanna for his continuous guidance and support during my Ph. D. study.
Besides my advisor, I also would like to express my sincere gratitude to the rest of
my advisory committee members: Dr. Robert A. Winholtz, Dr. Qingsong Yu and Dr.
Raghuraman Kannan, for their insightful comments and suggestions.
I would like to give my special thanks to my father, Chunqing Zhu, and my wife,
Tianyi Qiu for their consistent love, understanding, and support during my study.
I am grateful to my colleagues, Ajit Tambvekar and Ha T. T. Phan for their help in
the experiments.
I am also grateful to the technical staff of Engineering Technical Services (ETS):
O.S. “Rex” Gish, Brian Samuels and Rich Oberto, for their assistance in sample
machining and equipment repairing.
Financial support from U.S. Department of Homeland Security is gratefully
acknowledged.
iii
TABLE OF CONTENTS
FABRICATION AND CHARACTERIZATION OF NOVEL TRANSPARENT
LAMINATED GLASSCOMPOSITE PANELS FOR DYNAMIC LOAD
MITIGATION .....................................................................................................................i
ACKNOWLEDGEMENTS ............................................................................................. ii
TABLE OF CONTENTS ................................................................................................ iii
LIST OF FIGURES ........................................................................................................ vii
LIST OF TABLES ............................................................................................................. x
ABSTRACT .......................................................................................................................xi
CHAPTER 1 INTRODUCTION ...................................................................................... 1
1.1 Problem statement ...................................................................................................... 1
1.2 Literature reviewblast and its hazards ...................................................................... 2
1.2.1 Blast and blast effect on structures ..................................................................... 2
1.2.2 Blast hazards ....................................................................................................... 4
1.3 Literature reviewlaminated glass .............................................................................. 6
1.4 Literature reviewglass fiberreinforced polymer composite .................................... 9
1.4.1 Polymer composite ............................................................................................. 9
1.4.2 Glass fiberreinforced polymer composite ....................................................... 12
1.4.2.1 Polymer matrix........................................................................................... 14
1.4.2.2 Glass fiber .................................................................................................. 18
1.4.2.3 Summary .................................................................................................... 18
1.5 Literature reviewdynamic response of laminated plates under blast loading ......... 19
1.6 Summary .................................................................................................................. 22
CHAPTER 2 A NOVEL OPTICALLY TRANSPARENT WOVEN GLASS FIBER
REINFORCED POLYMER COMPOSITE: FABRICATION AND PROPERTIES30
iv
2.1 Introduction .............................................................................................................. 30
2.2 Experimental methods ............................................................................................. 32
2.2.1 Polyester plate fabrication ................................................................................ 32
2.2.2 Glass fiberreinforced composite fabrication ................................................... 33
2.2.3 Laminated glass panel fabrication .................................................................... 34
2.2.4 Refractive index measurement .......................................................................... 35
2.2.5 Light transmittance measurement ..................................................................... 36
2.2.6 Composite interlayer’s quasistatic mechanical properties testing ................... 36
2.2.6.1 Young’s modulus and Poisson’s ratio........................................................ 36
2.2.6.2 Shear modulus ............................................................................................ 38
2.2.7 Fracture toughness testing ................................................................................ 38
2.2.8 Dynamic mechanical properties testing ............................................................ 41
2.2.9 Fiber volume fraction determination ................................................................ 44
2.2.10 Blast resistance testing .................................................................................... 45
2.3 Theoretical model for light transmission through woven glass fiberreinforced
composite ....................................................................................................................... 47
2.4 Results and discussion ............................................................................................. 51
2.4.1 Effects of chemical additives on the refractive index of polyester ................... 51
2.4.1.1 Effect of methyl ethyl ketone peroxide (MEKP) concentration on the
refractive index of polyester .................................................................................. 51
2.4.1.2 Effect of cobalt (II) 2ethylhexanoate (CE) concentration on the refractive
index of polyester ................................................................................................... 52
2.4.1.3 Effect of divinylbenzene (DV) concentration on the refractive index of
polyester ................................................................................................................. 54
2.4.1.4 Effect of phenanthrene (PT) concentration on the refractive index of
polyester ................................................................................................................. 55
v
2.4.2 Light transmittance ........................................................................................... 57
2.4.2.1 Light transmittance of the composite interlayer ........................................ 57
2.4.2.2 Light transmittance of the laminated glass ................................................ 60
2.4.3 Quasistatic mechanical properties ................................................................... 62
2.4.4 Fracture toughness ............................................................................................ 65
2.4.5 Dynamic mechanical properties ........................................................................ 69
2.4.6 Blast resistance testing results .......................................................................... 73
2.5 Summary .................................................................................................................. 77
CHAPTER 3 A STUDY OF THE DYNAMIC RESPONSE OF THE NOVEL
LAMINATED GLASS UNDER BLAST LOADING ................................................... 83
3.1. Introduction ............................................................................................................. 83
3.2. Blast resistance testing ............................................................................................ 83
3.3 Blast resistance testing results ................................................................................. 84
3.4 Numerical modeling of the dynamic response of the fabricated laminated glass
under blast loading ......................................................................................................... 86
3.5 Comparison between numerical and experimental results ....................................... 92
3.6 Laminated glass failure analysis .............................................................................. 97
3.7 Summary ................................................................................................................ 101
CHAPTER 4 NONLINEAR DYNAMIC ANALYSIS OF THE NOVEL
LAMINATED GLASS UNDER BLAST LOADING ................................................. 103
4.1 Introduction ............................................................................................................ 103
4.2 Numerical modeling and finite element modeling of the dynamic response the
fabricated laminated glass under blast loading ............................................................ 103
4.2.1 Numerical modeling ....................................................................................... 103
4.2.2 Finite element modeling ................................................................................. 113
vi
4.3 Results and discussions .......................................................................................... 115
4.3.1 Midpoint deflection ......................................................................................... 115
4.3.2 Midpoint maximum principal stress history ................................................... 116
4.4 Summary ................................................................................................................ 122
CHAPTER 5 CONCLUSIONS AND FUTURE WORK ........................................... 126
APPENDIX A ................................................................................................................. 129
VITA................................................................................................................................ 135
vii
LIST OF FIGURES
Figure Page
1.1 Shock front expanding process ..................................................................................... 3
1.2 Glass fragments produced in Oklahoma City bombing. ............................................... 5
1.3 Laminated glass window and door fractured but remaining in frame in Oklahoma City
bombing. ............................................................................................................................. 6
1.4 Synthesis process of polyvinyl butyral (PVB) .............................................................. 7
1.5 Polymer composites classification .............................................................................. 10
1.6 Thermosetting resins market share in composites industry ....................................... 17
1.7 Tensile strength and modulus comparison among three resins ................................. 17
2.1 Mold for fabricating polyester and glass fiberreinforced composite plates .............. 33
2.2 Laminated glass structure ........................................................................................... 35
2.3 Shape and dimensions of tensile test specimens ......................................................... 37
2.4 Jintegral curve around a crack (notch) ...................................................................... 40
2.5 Dimensions of singleedgenotchedtension specimens ............................................. 41
2.6 Split Hopkinson bar (SHB) apparatus......................................................................... 43
2.7 Schematic of main components of a SHB system ...................................................... 43
2.8 Blast Load Simulator (BLS) ....................................................................................... 46
2.9 Glass panel installation inside the BLS ...................................................................... 46
2.10 Phase of light after passing through a glass fiber ..................................................... 47
2.11 Light transmission model of woven glass fiberreinforced composite ..................... 50
2.12 Refractive index of polyester (cured product) with different MEKP concentrations 52
2.13 Refractive index of polyester (cured product) with different CE concentrations ..... 53
viii
2.14 Refractive index of polyester (cured product) with different DV concentrations .... 55
2.15 Refractive index of polyester (cured product) with different PT concentrations ..... 56
2.16 Comparison between experimentally measured light transmittance and theoretically predicted light transmittance ........................................................................ 58
2.17 Readability of text through the glass fiberreinforced composite plate and the
polyester plate ................................................................................................................... 60
2.18 Light transmittance spectrum of the laminated glass ................................................ 61
2.19 Appearance of the fabricated laminated glass .......................................................... 62
2.20 Stressstrain curves of the glass fiberreinforced composites ................................... 63
2.21 Stress vs. strain curves of the composites in the initial linear region ....................... 64
2.22 Shear stressstrain curves of the glass fiberreinforced composites ......................... 64
2.23 Loaddisplacement curves for fiberreinforced composite specimens with different
initial crack lengths ........................................................................................................... 66
2.24 Strain energy per unit thickness versus initial crack length at different displacements
........................................................................................................................................... 68
2.25 Jintegral curves of the composite ............................................................................ 69
2.26 Stressstrain curves of the glass fiberreinforced composite at different strain rates 71
2.27 Effect of strain rate on compressive strength of the glass fiberreinforced composite
........................................................................................................................................... 72
2.28 Surface micrographs of the glass fiberreinforced composite at different strain rates
........................................................................................................................................... 73
2.29 Laminated glass window panel was cracked after the GSA level E blast test. Both
the outer surfaces of the glass plies were smooth to touch and minor damage to the
composite interlayer .......................................................................................................... 75
2.30 Level E blast loading resulted in severe damage to the window panel .................... 76
2.31 Thicker glass window panel after Level E blast loading .......................................... 76
ix
3.1 Pressuretime curve of the medium intensity blast ..................................................... 84
3.2 Midpoint deflection of the laminated glass under the medium intensity blast ........... 85
3.3 Pressuretime curve of the high intensity blast ........................................................... 85
3.4 Midpoint deflection of the laminated glass under the high intensity blast ................. 86
3.5 Schematic diagram of the laminated glass .................................................................. 88
3.6 The maximum deflection state of the laminated glass under the medium intensity
blast loading ...................................................................................................................... 93
3.7 The maximum deflection state of the laminated glass under the high intensity blast
loading............................................................................................................................... 94
3.8 Midpoint deflection of the laminated glass under the medium intensity blast loading
in the first deflection peak region ..................................................................................... 96
3.9 Midpoint deflection of the laminated glass under the high intensity blast loading in
the first deflection peak region ......................................................................................... 96
3.10 Midpoint maximum principal stress history under the medium intensity blast loading
........................................................................................................................................... 99
3.11 Midpoint maximum principal stress history under the high intensity blast loading 100
4.1 Schematic diagram of the laminated glass ................................................................ 104
4.2 SHELL181 geometry ............................................................................................... 114
4.3 Shell section page ..................................................................................................... 114
4.4 Midpoint deflection comparison .............................................................................. 116
4.5 Midpoint maximum principal stress history of the inner glass surface .................... 118
4.6 Midpoint maximum principal stress history of the outer glass surface .................... 118
4.7 Comparison of midpoint deflections under the medium intensity blast loading ...... 120
4.8 Comparison of midpoint maximum principal stresses (inner surface) ..................... 121
4.9 Comparison of midpoint maximum principal stresses (outer surface) ..................... 122
x
LIST OF TABLES
Table Page
1.1 Properties of fibers ..................................................................................................... 11
1.2 Cost of fibers .............................................................................................................. 12
1.3 Price of resins .............................................................................................................. 18
2.1 Some properties of glass fibers and polyester............................................................. 34
2.2 Candidate formulations for making the optically transparent composite ................... 57
2.3 Quasistatic mechanical properties of the glass fiberreinforced composites ............. 65
2.4 Dynamic mechanical properties of the glass fiberreinforced composite ................... 71
xi
ABSTRACT
Bomb threats and attacks are common in many parts of the world today. One of the
significant effects of a blast is damage to the glass windows in nearby buildings. The
debris produced from the damaged windows, especially the sharp glass fragments
produced, can lead to severe injuries and even casualties. One way to mitigate the
damage is to use blastresistant laminated glass, which is conventionally made of one or
more polyvinyl butyral (PVB) interlayer sandwiched between two or more glass sheets,
for windows. Although the PVB interlayer is widely used in the world, it still has some
disadvantages, such as low strength to weight ratio which results in large thickness and
increased weight of the laminated glass. The low strength to weight ratio problem can be
solved by replacing the PVB interlayer with a transparent glass fiberreinforced polymer
composite interlayer, because glass fiberreinforced composites have high strength to
weight ratio and potentially higher fracture toughness. By using the glass fiberreinforced
composite interlayer, the thickness and weight of the laminated glass can be potentially
reduced.
A laminated glass panel utilizing a newly developed transparent glass fiber
reinforced composite interlayer has been fabricated in this study. The transparent
composite interlayer was obtained by matching the refractive index of the polyester resin
matrix with that of Eglass fibers. The light transmittance of the fabricated laminated
glass is above 60% over the light wavelength range of 482 nm to 700 nm with the highest
transmittance is 84.4% when the light wavelength is 577 nm. The composite interlayer’s
mechanical properties under both quasistatic and dynamic loading conditions have been
xii
characterized. In addition, the fabricated glass panels were tested under various blast
loading conditions. The panels perform well under U.S. General Services Administration
(GSA) specified C, D and E blast loading levels.
In this research, the dynamic response, in terms of the midpoint deflection, of the
fabricated laminated glass under blast loading has been analytically investigated using
modelbased method and finite element method. Failure analysis of the laminated glass
was performed using the stress analysis approach.
1
CHAPTER 1 INTRODUCTION
1.1 Problem statement
Bomb threats and attacks are now common in many parts of the world. One of the
significant effects of a blast is damage to the glass windows in nearby buildings. The
sharp glass fragments produced from the damaged windows can lead to large casualties.
And blast pressure entering buildings through the damaged windows can cause additional
injuries to the occupants. So the need of mitigating the hazards caused by windows
failure is essential.
One way to mitigate the damage is to use blastresistant laminated glass, which is
conventionally made of one or more polyvinyl butyral (PVB) interlayer sandwiched
between two or more glass sheets, for windows. PVB is chosen as the interlayer material
mainly due to its optical transparency. Although laminated glass with PVB interlayer is
widely used in the world, it still has some disadvantages, such as large thickness
requirement for blast resistance, which increases the production cost and installation cost.
The thickness and weight can be potentially reduced by replacing the PVB interlayer with
a glass fiberreinforced polymer composite interlayer, because glass fiberreinforced
polymer composites have high strength to weight ratio.
Typically glass fiberreinforced polymer composites are opaque. The low
transparency (light transmittance) is due to the refractive index mismatch between glass
fibers and the polymer matrix. The transparency increases with the decrease of the
refractive index difference. However, only a basic understanding of the relationship
2
between the transparency and the refractive index difference is available. A quantitative
understanding of the relationship is needed.
A study of the dynamic response of a blastresistant laminated glass under blast
loading is important for understanding the effect of blast loading on the laminated glass.
Although the dynamic response of the laminated glass with PVB interlayer under blast
loading has been widely studied, the dynamic response of the laminated glass with glass
fiberreinforced polymer composite interlayer under blast loading has not been studied
yet. So, such a study is needed.
This research focuses on fabricating a laminated glass panel utilizing a transparent
glass fiberreinforced polymer composite interlayer. The transparency of the composite
interlayer is achieved by matching the refractive index of the polymer matrix with that of
glass fibers. The relationship between the transparency and the refractive index difference
is quantitatively studied. The dynamic response of the fabricated laminated glass under
blast loading is also investigated.
1.2 Literature reviewblast and its hazards
1.2.1 Blast and blast effect on structures
A blast is a sudden release of stored energy. When a blast happens, rapid expansion
of energy resulting from the blast gives rise to a wave of compressed air which is called
shock front. The shock front travels radially in air in all directions. As the shock front
moves, the shock front releases energy to surrounding air and the overpressure of the
shock front decreases. When the pressure of the shock front drops below the atmospheric
3
pressure, surrounding air gives energy to the shock front and the pressure of the shock
front finally returns to the atmospheric pressure [1]. The whole process is shown in Fig.
1.1 [2].
Timetp
Atmospheric
pressure
Pa
Pm
Po=
PmP
a
Figure 1.1 Shock front expanding process
The pressuretime curve shown in Fig. 1.1 can be described using the following
equation [3]
 /= 1 / e (1.1)pt t
o pP t P t t
where P(t) is the blast pressure at time t, Po is the peak pressure, is a constant and tp is
the positive pressure duration time. According to references [3, 4], the key parameters of
a blast are: peak pressure Po, constant and positive pressure duration time tp.
Blast effect on structures can be divided into three types. In the first type, the shock
front is stopped by a relatively small structure. In this case, blast wave simultaneously
4
acts on the entire structure and the structure is massive enough to resist translation. In the
second type, the shock front is stopped by a structure which is much smaller than the
structure in the first case. In this case, blast wave also simultaneously acts on the entire
structure but the structure is small enough to be moved by the blast wave. In the final
type, the shock front is stopped by a big structure. The shock front is too small to act on
the whole structure simultaneously. Instead of simultaneously loading, the structure is
affected in succession [5].
1.2.2 Blast hazards
Every year, numerous blast events take place in the United States. These blasts are
usually small blast events (explosive weights are equal or less than 10 lb (4.53 kg) TNT
(2, 4, 6trinitrotoluene)) [6]. The damage caused by such blasts is small. However, large
blasts occur infrequently, such as bombing in Oklahoma City, Oklahoma [7], the first
bomb attack on the World Trade Center, New York City, New York [8], bombing in
Manchester City, England [9] and attack on Embassy of Australia in Jakarta, Indonesia
[10]. For those blasts, 1000 lb (453 kg) or more explosives were used. Under such blast
loadings, experience shows that the most damage occurs to the windows of surrounding
buildings [11]. Windows, which are made of ordinary glass, usually break into pieces in
such situations (Fig. 1.2). The broken pieces can travel at a speed up to 200 ft/sec (61
m/s) [12], which can cause great injuries and even deaths [7, 13]. In the Oklahoma City
bombing, 508 persons suffered injuries outside the Alfred P. Murrah building (the
attacked building) [6]. Of these, 200 injuries were directly related to the broken glass
5
fragments. In addition to glass fragments, blast pressure passing through the broken
windows may cause additional injuries because it only needs 15 psi (~100 kPa) pressure
to rupture eardrums and cause lung damage and pressure created by an explosion can be
very high (higher than 15 psi) [14]. Hence, the need of mitigating the hazards caused by
windows failure is essential. One way to mitigate the damage is to use laminated glass for
windows. Using laminated glass can significantly reduce the possibility of generating
fragments during a blast loading (Fig. 1.3).
Figure 1.2 Glass fragments produced in Oklahoma City bombing (Reprinted with permission from “Survey
of window glass broken by Oklahoma City bomb on April 19, 1995, revised”, copyright belongs to Glass
Research and Testing Laboratory, Texas Tech University).
6
Figure 1.3 Laminated glass window and door fractured but remaining in frame in Oklahoma City bombing
(Reprinted with permission from “Survey of window glass broken by Oklahoma City bomb on April 19,
1995, revised”, copyright belong to Glass Research and Testing Laboratory, Texas Tech University).
1.3 Literature reviewlaminated glass
Laminated glass, which is normally used in the places where human injury may
happen [2, 15, 16] or where glass may fall if shattered [17], was invented in 1910 by a
French chemist Edouard Benedictus [18], who first patented the use of gelatin as the
interlayer between glass sheets. Gelatin interlayer binds two normal glass sheets together
and this glass “sandwich” looks like normal glass and behaves as a single unit.
The glass sheets used to make laminated glass are usually tempered glass sheets.
Tempered glass is produced by first heating annealed glass (the most common glazing
material used in residential windows) and then rapidly cooling the glass. This treatment
gives additional strength to the glass. So, tempered glass is stronger than annealed glass
7
of the same dimension. The typical tensile strength of tempered glass (more than 175
MPa) is much higher than that of annealed glass (around 40 MPa) [15, 19]. Another
advantage of tempered glass is that tempered glass tends to break into relatively small
and blunt edges fragments under external loading. This reduces the possibility of injury to
people. Therefore, instead of annealed glass, tempered glass is chosen to make the
laminated glass in this study.
With the development of technique, instead of gelatin, the interlayer of modern
laminated glass is made of polyvinyl butyral (PVB). Polyvinyl butyral (PVB) is a resin
used for applications that require optical transparency, strong binding, high toughness
and high flexibility [20]. PVB is prepared by reacting polyvinyl alcohol with
butyraldehyde. The synthesis process of PVB is shown in Fig. 1.4.
CH
OH
CH2 CH CH2
OH
+ CH3 CH2 CH2 CHO
H+H2O
CH2
CH CH
O O
CH
CH2
CH2
CH3
CH2x
Figure 1.4 Synthesis process of polyvinyl butyral (PVB)
Polyvinyl alcohol Butyraldehyde
Polyvinyl butyral
8
PVB has many applications, such as solar modules [21] and ceramic binders [22].
The major application of PVB is for fabricating the interlayer of laminated glass. The
reason for using PVB as the interlayer is: firstly, PVB is colorless; secondly, PVB
interlayer can bind the resulting glass fragments when the outer layer glass sheets are
broken; Last but not least, PVB has good energy absorption ability which is due to its
plastic deformation after impacting.
Currently, PVB is a mature product and is provided by a number of companies,
including Chung Petrochemicals (“WINLITE” brand PVB, Taiwan), Sekisui (“SLec”
brand PVB, Japan), DuPont (“Butacite” brand PVB, United States), Eastman (“Saflex”
brand PVB, United States) and Kuraray Europe GmbH (“Trosifol” brand PVB and
“Mowital/Pioloform” brand PVB, Germany) [20].
Besides PVB, there are other types of interlayer materials in use, including
transparent thermoplastic polyurethane (TPU) [23] and transparent polycarbonate (PC)
[24].
Transparent TPU is a kind of polyurethane which has high optical clarity and
excellent adhesion property to glass. TPU also offers excellent resistance to hydrocarbon
oil, chemicals and moisture [25]. The combination of these features enables the laminated
glass designers to use it as the interlayer of laminated glass. The shortcoming of TPU is
its low mechanical properties. For example, the Young’s modulus of TPU is around 60
MPa (at room temperature (~20 ºC)) [26], which is much lower than that of PVB (~100
MPa at room temperature (~20 ºC)) [27]. Because of its low mechanical properties, the
9
impact resistance of the laminated glass with TPU interlayer is lower than that of the
laminated glass with PVB interlayer.
PC is a thermoplastic polymer. Compared with other transparent polymers, the
advantage of PC is that it is very tough [24, 28]. If a blast happens near a laminated glass
with PC interlayer and the outer layer glass sheets of the laminated glass shatter, the PC
interlayer may be able to prevent the penetration of debris by bulging plastically [29].
The main problem for PC, which is not a big problem for PVB, is that it embrittles with
age. The embrittlement is due to 1) physical aging (thermodynamic equilibrium) [30], 2)
chemical changes due to exposure to ultraviolet (UV) light, ozone, nitrogen oxides,
moisture, etc. [3135], 3) physical damage, e.g. surface microcracks introduced by solar
radiation [36].
Compared with TPU (low mechanical properties) and PC (aging problem), it can be
noted that PVB is a better interlayer material for laminated glass. But PVB is not the
perfect interlayer material, it has some drawbacks, such as relatively low strength to
weight ratio. According to literatures [3740], glass fiberreinforced polymer composite
materials possess high strength to weight ratio. Therefore glass fiberreinforced polymer
composite is a potential replacement for PVB.
1.4 Literature reviewglass fiberreinforced polymer composite
1.4.1 Polymer composite
Polymer composite materials are engineering materials made from two or more
materials. The major advantages of polymer composite materials are that they have high
10
strength to weight ratio, are economical, light in weight, weather resistant, chemical
resistant and corrosion resistant. A polymer composite is composed of reinforcement and
polymer matrix. The matrix holds the reinforcement to form a material with better
properties. Based on the form of reinforcement, polymer composites can be classified as
fiberreinforced composite, particlereinforced composite, flakereinforced composite and
fillerreinforced composite (Fig. 1.5). Compared with other composites, fiberreinforced
polymer composite, especially woven fiberreinforced composite, doesn’t have the
reinforcement agglomeration problem which may lead to the decrease of strength [41
43]. So, fiberreinforced composite is the most widely used polymer composite.
Particlereinforced compositeFiberreinforced composite
Flakereinforced composite Fillerreinforced composite
Figure 1.5 Polymer composites classification
11
For fiberreinforced composite, the most commonly used fibers are glass fibers,
aramid fibers and carbon fibers. The properties and cost of these fibers are listed in Table
1.1 and Table 1.2 respectively. From Table 1.1, it can be observed that all these fibers
have good mechanical properties. From Table 1.2, it can be noted that the price of aramid
fibers and carbon fibers is much higher than that of glass fibers. Because of the price
advantage, glass fiber is the most widely used reinforcement material.
Table 1.1 Properties of fibers [44]
Material E, GPa b , GPa , 103 kg/m
3 /E , MJ/kg /b , MJ/kg
Eglass
Sglass
Aramid
HS carbon
HM carbon
70
85
124
253
520
2.4
4.5
3.6
4.5
2.4
2.54
2.49
1.44
1.8
1.85
28.5
34.3
86
140
281
0.95
1.8
2.5
2.5
1.3
E is Young’s modulus, b is tensile strength, is density, HS carbon is the high strength carbon and HM
carbon is the high modulus carbon.
12
Table 1.2 Cost of fibers [15, 45]
Material Cost, $/kg
Eglass
Sglass
Aramid
HS carbon
HM carbon
~2.2
~20
~50
70200
150600
1.4.2 Glass fiberreinforced polymer composite
Glass fiberreinforced polymer composite is a composite made of polymer matrix
and glass fibers reinforcement. Incorporation of glass fibers into polymer matrix can
greatly improve the mechanical properties of the polymer matrix.
Abdulmajeed et al. [46] found the mechanical properties of glass fiberreinforced
poly(triethyleneglycol dimethacrylate (TEGDMA)) could be enhanced by increasing the
volume fraction of glass fibers. By increasing the volume fraction of glass fibers from
51.7% to 61.7%, there was an increase of 27% in Young’s modulus, 34% in toughness,
15% in load bearing capacity and 8% in flexural strength.
Akkapeddi reported [47] that by incorporating 15 wt% of glass fibers in a polyamide
nanocomposite, flexural modulus of the composite was increased by 49%, flexural
strength was increased by 18%, tensile strength was increased by 30% and impact
toughness was increased by 100%.
Iba et al. [48] fabricated a glass fiberreinforced epoxy matrix polymer composite.
They found Young’s modulus of the composite increased with the increase of the fiber
13
volume fraction. Young’s modulus increased linearly from about 4 GPa to 36 GPa with
the fiber volume fraction increasing from 0% to 50%. They also found that the tensile
strength of the composite increased linearly with the increase of the fiber volume
fraction. They concluded that incorporation of glass fibers into the epoxy matrix could
improve the mechanical properties of the epoxy matrix. Although adding glass fibers
could improve the mechanical properties of the epoxy matrix, the authors reported that
adding glass fibers decreased the transparency (light transmittance) of the epoxy matrix.
They believed this is caused by the refractive index mismatch between glass fibers and
the polymer matrix.
To sum up, adding glass fibers into a polymer matrix can greatly improve its
mechanical properties, but the transparency of the glass fiberreinforced polymer
composite decreases due to the refractive index mismatch between glass fibers and the
polymer matrix.
Iba et al. [49] reported that when glass fiber volume fraction was 10%, with the
refractive index difference increased from 0.0005 to 0.0015, the light transmittance, at the
light wavelength of 589 nm, of a glass fiber reinforced epoxy composite decreased from
80% to 10%.
Olson et al. [37] tested the optical transparency of a glass fiberreinforced poly
(methyl methacrylate) (PMMA) composite. They found that the light transmittance of the
composite decreased with the increase of the volume percentage of glass fibers. They
stated that the reason for the reduction in the transmittance is due to the presence of more
reflection interfaces (introduced by the presence of glass fibers) in the composite. If the
14
refractive index of glass fibers approaches that of the polymer matrix, the reflection will
decrease. If glass fibers’ refractive index is the same as the polymer matrix’s refractive
index, the reflection will be eliminated. In this situation, the number of fibers cannot
affect the light transmittance of the composite and the composite will behave as an
optically transparent material. Authors believed that good refractive index match between
glass fibers and the PMMA matrix could increase the light transmittance (transparency)
of the fiberreinforced PMMA composite.
Lin et al. [50] thought the light transmittance of a glass fiberreinforced composite
depends upon the light extinction coefficient of the composite. The coefficient is a
function of several factors: (a) the ratio of the refractive indices of glass fibers and
polymer matrix; (b) the fiber content; (c) the distribution in the refractive index of fibers;
(d) the fiber diameter; and (e) the amount of fibers not wetted by the polymer matrix. To
achieve the highest light transmittance, glass fibers’ refractive index should match the
matrix’s refractive index. They found the refractive index of glass fibers could be
changed by annealing. According to this discovery, they fabricated a transparent glass
fiberreinforced PMMA composite by matching the refractive index of glass fibers with
that of the PMMA matrix through changing the annealing condition of glass fibers.
1.4.2.1 Polymer matrix
Plastic resins are commonly used as the matrix of glass fiberreinforced polymer
composites [5154]. According to property differences, plastic resins can be divided into
two groups, one is thermosetting plastic resins, and the other is thermoplastic plastic
15
resins. Thermosetting resin is the resin which is liquid before curing and is solid after
curing. The cure can be done through heat, irradiation or chemical reactions [15].
Thermoplastic resin is the resin which is soft above a specific temperature and is hard
below this temperature. Compared with thermoplastic resins, thermosetting resins, such
as polyester, epoxy and vinyl ester, are more often used as the matrix materials. Because
thermosetting resins are liquid at room temperature, this allows for convenient
impregnation of glass fibers. Thermoplastic resins are usually solid at room temperature,
so it is very difficult to impregnate glass fibers into thermoplastic resins. In order to make
a thermoplastic fiberreinforced composite, following procedures are used: 1) heat the
matrix resin to its melting point; 2) impregnate fibers into the matrix; 3) cool the
composite to room temperature (~20 ºC). This process is more complex and expensive
than a thermosetting fiberreinforced composite manufacturing process.
Polyester resin is the main matrix material for thermosetting fiberreinforced
polymer composite manufacture. It is a kind of polymer which contains ester functional
group in the main chain. From Fig. 1.6, it can be seen that polyester resin holds 66%
share of thermosetting resins used in composite industry [55]. Polyester is cheap, easy to
use and compatible with glass fibers [15, 56].
Epoxy resin is another source for thermosetting fiberreinforced polymer composite
manufacture. Epoxy resin is a class of reactive polymers which contain epoxide groups.
Epoxy resin contributes 23% share of thermosetting resins used in composite industry
[55]. The annual output value of epoxy resin is very large. As of 2009, the output value of
epoxy industry is more than 5 billion dollars in North America and about 15.8 billion
16
dollars worldwide [57]. The applications of epoxy resins are extensive and including
adhesives, coatings and composite matrices. Epoxy has good mechanical properties,
water resistance and high temperature resistance [58, 59].
Vinyl ester resin is the third often used matrix material for thermosetting fiber
reinforced polymer composite manufacture. Vinyl ester resin is manufactured by
esterification of an epoxy resin with an unsaturated carboxylic acid. This resin is created
like infusing epoxy molecules into polyester molecules. So, vinyl ester resin possesses
both attributes of epoxy and polyester resins. Vinyl ester resin contributes around 5%
share of thermosetting resins used in composites industry [55]. Vinyl ester resin has good
water corrosion resistance, so it is the commonly used resin in marine industry.
From Fig. 1.7, it can be observed that among three resins, the properties of the
epoxy resin are the best and the properties of the vinyl ester resin and the polyester resin
are similar. From table 1.3, it can be observed that the price of polyester is the lowest.
Consider costperformance ratio, polyester is chosen as the matrix material in this
research.
17
Figure 1.6 Thermosetting resins market share in composites industry (2007) [55]
Figure 1.7 Tensile strength and modulus comparison among three resins [60]
Polyester, 66%
Epoxy, 23%
Vinyl ester, 5%
Others, 6%
0
10
20
30
40
50
60
70
Polyester Vinyl ester Epoxy
Ten
sile
Str
ength
(M
Pa)
0
0.5
1
1.5
2
2.5
3
3.5
4
Polyester Vinylester Epoxy
Ten
sile
Mo
dulu
s (G
Pa)
18
Table 1.3 Price of resins
Resin Name Price ($/Ton)
Polyester
Epoxy
~1800 (FOB)* [61]
~3000 (FOB) [62]
Vinyl ester ~2400 [63]
*FOB price: free on board price.
1.4.2.2 Glass fiber
Sglass fiber and Eglass fiber are the most commonly used glass fibers. Eglass
fiber is a kind of glass fiber which has high strength, high stiffness, good chemical
resistance and good electric insulation properties. Compared with Eglass fiber, Sglass
fiber is a kind of glass fiber which has better mechanical properties (Table 1.1). But E
glass fiber is much cheaper than Sglass fiber (Table 1.2). By considering cost
performance ratio, Eglass fiber is chosen as the reinforcement in this research.
1.4.2.3 Summary
In this research, glass fiberreinforced composite, which is intended to be used as the
interlayer of a blastresistant laminated glass panel, will be fabricated using polyester
(matrix) and Eglass fibers (reinforcement). The outer layer glass sheets of the blast
resistant laminated glass panel are tempered glass sheets.
The primary use of blastresistant laminated glass (or other laminated plates) is to
protect people from injuries under blast/impact loading conditions. Therefore, the
response of a laminated glass (or other laminated plates) under dynamic loading is a very
19
important criterion for measuring the suitability of the laminated glass (or other laminated
plates).
1.5 Literature reviewdynamic response of laminated plates under blast
loading
Much work has been done to understand the effect of dynamic loading, such as
small missile impact loading and blast loading, on laminated plates such as laminated
glass and laminated polymer composite.
Ji et al. [64] studied the probability of damage at the impact site of laminated glass
units under low velocity small missile impact loading. A numerical model was introduced
to characterize the probability of damage. According to their report, the probability of
damage at the impact site could be predicted by the developed numerical model.
Calculated results were in good agreement with the experimental results.
Kaiser et al. [65] presented experimental results of low velocity, small steel ball
impact tests on laminated glass plates with polyvinyl butyral (PVB) interlayer. Their
results showed that increasing the interlayer thickness and increasing the inner glass sheet
thickness could significantly increase the steel ball impact velocity required to break the
inner glass sheet.
Larcher et al. [66] experimentally studied the response of impactloaded laminated
glass with PVB interlayer. They conducted their experiments at a shock tube facility.
Besides experiments, they also used several numerical models, such as layered model and
solid 3D model, to simulate the response of the impactloaded laminated glass. They
20
found that the layered model could efficiently simulate the experimentally measured
results, also in cases where the interlayer failed. The 3D solid model could also simulate
the experimental results, though requiring larger computational power. Lusk et al. [67]
also experimentally studied the response of impactloaded laminated glass with PVB
interlayer. Three samples were tested using a fullscale shock tube. Instead of numerical
modelling, Lusk used the commercial finite element code LSDYNA to simulate the
dynamic response of the laminated glass. The results simulated by LSDYNA agreed
well the experimentally measured results. Lusk stated that the mechanical properties of
the materials that were used to fabricate the laminated glass were the most important
parameters for LSDYNA inputs and should be tested before simulation.
Turkmen et al. [68] performed blast tests on a stiffened laminated plate (carbon fiber
fabric) and measured blast pressures and strains at different points on the stiffened
laminated plate and its stiffener. After analyzing the measured strain data, Turkmen
stated that the peak strain of the laminated plate depended on the peak pressure value and
the strain variation with time depended on the pressure variation with time. The authors
also numerically modelled the response of the plate and reported the numerical results
correlated well with the experimental results.
Wei et al. [2, 69, 70] investigated the dynamic response of laminated glazing with
PVB interlayer subjected to blast loading through theoretical approaches. They presented
two models, which are based on the classical small deflection plate theory and von
Karman’s large deflection plate theory, respectively, to characterize the response of the
laminated glass under blast loading. For comparison, they also simulated the dynamic
21
response using a 3D finite element code LSDYNA. The modelpredicted results matched
with the finite element analysis results. The authors also studied the damage probability
of the laminated glass subjected to blast loading. Their results showed that newly
fabricated laminated glass panel could withstand higher blast loading than old ones and
decreasing outer glass sheet thickness and increasing inner glass sheet thickness while
keeping the total thickness of the laminated glass constant is an economical way to
increase the blast resistance of the laminated glass.
Amadio et al. [71] visited the problem of the behavior of a conventional glazing
structure (glass curtain wall) subjected to high and lowlevel air blast loading. The
authors found that additional deformability and additional energy dissipation ability could
be provided to the conventional glass curtain wall by adding viscoelastic (VE) devices at
the frame corners of the glass curtain wall. The VE device was made of two metallic
plates and a middle rubber (viscoelastic material) layer. VE devices were positioned
between the frame of the glass curtain wall and the structural backup of it. The authors
discovered that VE devices could reduce the maximum stresses in the glass curtain wall,
reduce the deflection of the total structure and decrease the maximum reactions
transmitted to the structural backup.
Birman et al. [72] studied the dynamic response of simply supported anti
symmetrically laminated angleply thick plates (graphiteepoxy plates) subjected to blast
loading. A closedform solution was proposed for describing the dynamic response of the
plates. In their work, the effect of transverse shear deformations on the response of the
plates was considered. Their analysis yielded a nondimensional deflection versus time
22
relationship and this relationship was used to calculate the stresses and strains of the
plates.
Kazancı et al. [73] addressed the problem of nonlinear dynamic response of a simply
supported laminated plate (fiberglass fabric) under blast loading. They derived equations
of motion of the laminated plate, in the frame of von Karman’s deflection theory with the
consideration of geometric nonlinearity effects. The equations of motion were solved
using finite difference method and the obtained results were compared with literature and
finite element analysis results. Good agreement was reported for deflection and
frequencies of vibrations.
1.6 Summary
There has been a lot of research on methods to mitigate the damage caused by
windows failure under blast loading. Until today, the most effective method to mitigate
the damage is use blastresistant laminated glass for windows. Currently, the most widely
used laminated glass is the laminated glass with polyvinyl butyral (PVB) interlayer. The
reason for using PVB as the interlayer material has been mentioned previously: colorless;
able to bind glass fragments after windows failure; good energy absorption ability. The
disadvantage of the laminated glass with PVB interlayer is its large thickness and weight.
This disadvantage can be overcome by replacing the PVB interlayer with a transparent
glass fiberreinforced polyester composite interlayer which has high strength to weight
ratio. The transparency of the glass fiberreinforced composite is achieved by matching
the refractive index of the polymer matrix with that of glass fibers.
23
The dynamic response of the laminated glass with PVB interlayer under blast
loading has been experimentally and analytically studied. Several numerical models have
been developed to characterize the dynamic response of the laminated glass with PVB
interlayer under blast/dynamic loading. But to the best of our knowledge, the dynamic
response of the laminated glass with glass fiberreinforced composite interlayer under
blast loading has not been studied previously.
In this research, a novel blastresistant laminated glass panel utilizing a transparent
glass fiberreinforced composite interlayer has been successfully fabricated. The dynamic
response of the fabricated laminated glass under blast loading has been investigated
experimentally and analytically.
The investigation in this research has been organized in three parts:
(1) Part I: this part is the introduction, which includes Chapter 1 titled “Introduction”.
(2) Part II: this part focuses on fabricating the transparent glass fiberreinforced
composite interlayer and studying its optical properties and mechanical behavior, which
includes Chapter 2 titled “A novel optically transparent woven glass fiberreinforced
polymer composite: fabrication and properties”.
(3) Part III: this part reports studies of the dynamic response of the novel blast
resistant laminated glass under blast loading, which contains Chapter 3 titled “A study of
the dynamic response of the novel laminated glass under blast loading” and Chapter 4
titled “Nonlinear dynamic analysis of the novel laminated glass under blast loading”.
24
REFERENCES
[1] Smith, P.D., and Hetherington, J.G., 1994, "Blast and ballistic loading of structures",
Oxford: ButterworthHeinemann.
[2] Wei, J., and Dharani, L.R., 2006, "Response of laminated architectural glazing
subjected to blast loading", International Journal of Impact Engineering, 32, No.12,
pp.20322047.
[3] Kinney, G.F., and Graham, K.J., 1985, "Explosive shocks in air", Berlin and New
York: SpringerVerlag.
[4] Baker, W.E., 1973, "Explosions in air", Austin, TX: University of Texas Press.
[5] Forbes, D.J., 1999, "Blast loading on petrochemical buildings", Journal Energy
Engineering, 125, No.3, pp.94102.
[6] Norville, H.S., and Conrath, E.J., 2006, "Blastresistant glazing design", Journal of
Architectural Engineering, 12, No.3, pp.129136.
[7] Norville, H.S., Smith, M.L., and King, K.W., 1995, "Survey of window glass broken
by the Oklahoma City bomb on April 19, 1995", Lubbock, TX: Texas Tech University.
[8] Quenemoen, L.E., Davis, Y.M., Malilay, J., Sinks, T., Noji, E.K., and Klitzman, S.,
1996, "The World Trade Center bombing: injury prevention strategies for highrise
building fires", Disasters, 20, No.2, pp.125132.
[9] Wikipedia, "1996 Manchester bombing", http://en.wikipedia.org/wiki/1996_
manchester_bombing.
[10] Wikipedia, "2004 Australian Embassy bombing in Jakarta", http://en.wikipedia.org/
wiki/2004_Australian_Embassy_bombing_in_Jakarta.
[11] Smith, D., 2001, "Glazing for injury alleviation under blast loading—United
Kingdom practice", Glass Processing Days, pp.335340.
[12] Graham, "About blast mitigation", http://www.grahamwindows.com/blast/ about_
blast.html.
[13] Brismar, B., and Bergenwald, L., 1982, "The terrorist bomb explosion in Bologna,
Italy, 1980: an analysis of the effects and injuries sustained", The Journal of Trauma, 22,
No.3, pp.216220.
[14] Katz, E., Ofek, B., Adler, J., Abramowitz, H.B. and Krausz, M.M., 1989, "Primary
blast injury after a bomb explosion in a civilian bus", Annals of Surgery, 209, No.4,
pp.484488.
25
[15] Shankar, K.R., 2007, "Failure of transparent polymer composite laminated glass
panels under impact loading", Columbia, MO: University of Missouri.
[16] Xu, J., Li, Y., Liu, B., Zhu, M., and Ge, D., 2011, "Experimental study on
mechanical behavior of PVB laminated glass under quasistatic and dynamic loadings",
Composites Part B: Engineering, 42, No.2, pp.302308.
[17] Osborn, R.A., 1996, "Shedding light on skylights", Fine Homebuilding, 102, No.5,
pp.4853.
[18] Wikipedia, "Laminated glass", http://en.wikipedia.org/wiki/Laminated_glass.
[19] Zang, M., and Chen, S., 2012, "Laminated glass, Wiley Encyclopedia of
Composites", Hoboken , NJ: John Wiley & Sons.
[20] Wikipedia, "Polyvinyl butyral", http://en.wikipedia.org/wiki/Polyvinyl_butyral.
[21] Fonrodona, M., Santos, S., Mata, C., Vetter, M., and Andreu, J., 2010, "Performance
and productivity improvements in very large area amorphous silicon modules",
Proceedings of the 25th EUPVSEC, pp.36613664.
[22] Su, B., and Button, T., 2009, "A comparative study of viscous polymer processed
ceramics based on aqueous and nonaqueous binder systems", Journal of Materials
Processing Technology, 209, No.1, pp.153157.
[23] Folgar, F., "Advanced aliphatic polyurethane resins for high durability and superior
ballistic performance laminated glass", http://intermaterialsusa.com/images/FCKU
ploads/file/Advanced_AliphaticPolyurethanes_INTER_MaterialsLLC_1(2).pdf.
[24] Walley, S., Field, J., Blair, P., and Milford, A., 2004, "The effect of temperature on
the impact behaviour of glass/polycarbonate laminates", International Journal of Impact
Engineering, 30, No.1, pp.3153.
[25] Schollenberger, C., and Stewart, F., 1971, "Thermoplastic polyurethane hydrolysis
stability", Journal of Elastomers and Plastics, 3, No.1, pp.2856.
[26] Promolding, "TPU", http://promolding.nl/materiaalmunt.php?lan=uk&c=125.
[27] Bennison, S.J., Qin, M.H., and Davies, P.S., 2008, "Highperformance laminated
glass for structurally efficient glazing", Innovative LightWeight Structures and
Sustainable Facades, pp.112.
[28] Rietsch, F., and Bouette, B., 1990, "The compression yield behaviour of
polycarbonate over a wide range of strain rates and temperatures", European Polymer
Journal, 26, No.10, pp.10711075.
26
[29] Walley, S.M., Field, J.E., Blair, P.W., and Milford, A.J., 2004, "The effect of
temperature on the impact behaviour of glass/polycarbonate laminates", International
Journal of Impact Engineering, 30, No.1, pp.3153.
[30] Zurimendi, J., Biddlestone, F., Hay, J., and Haward, R., 1982, "Physical factors
affecting the impact strength of polycarbonate", Journal of Materials Science, 17, No.1,
pp.199203.
[31] Sherman, E., Ram, A., and Kenig, S., 1982, "Tensile failure of weathered
polycarbonate", Polymer Engineering & Science, 22, No.8, pp.457465.
[32] Clark, D.T., and Munro, H.S., 1984, "Surface and bulk aspects of the natural and
artificial photoageing of Bisphenol A polycarbonate as revealed by ESCA and difference
UV spectroscopy", Polymer Degradation and Stability, 8, No.4, pp.195211.
[33] Turton, T., and White, J., 2001, "Degradation depth profiles and fracture of UV
exposed polycarbonate", Plastics, Rubber and Composites, 30, No.4, pp.175182.
[34] Gardner, R.J., and Martin, J.R., 1979, "Humid aging of plastics: effect of molecular
weight on mechanical properties and fracture morphology of polycarbonate", Journal of
Applied Polymer Science, 24, No.5, pp.12691280.
[35] Factor, A., and Chu, M., 1980, "The role of oxygen in the photoageing of bisphenol
A polycarbonate", Polymer Degradation and Stability, 2, No.3, pp.203223.
[36] Blaga, A., and Yamasaki, R., 1976, "Surface microcracking induced by weathering
of polycarbonate sheet", Journal of Materials Science, 11, No.8, pp.15131520.
[37] Olson, J.R., Day, D.E., and Stoffer, J.O., 1992, "Fabrication and mechanical
properties of an optically transparent glass fiber/polymer matrix composite", Journal of
Composite Materials, 26, No.8, pp.11811192.
[38] Novak, B.M., 1993, "Hybrid nanocomposite materials—between inorganic glasses
and organic polymers", Advanced Materials, 5, No.6, pp.422433.
[39] Mohd, I.Z., Leong, Y., Steeg, M., and Karger, K.J., 2007, "Mechanical properties of
woven glass fabric reinforced in situ polymerized poly (butylene terephthalate)
composites", Composites Science and Technology, 67, No.3, pp.390398.
[40] Malchev, P.G., David, C.T., Picken, S.J., and Gotsis, A.D., 2005, "Mechanical
properties of short fiber reinforced thermoplastic blends", Polymer, 46, No.11, pp.3895
3905.
[41] Mollazadeh, S., Javadpour, J., and Khavandi, A., 2007, "Biomimetic synthesis and
mechanical properties of hydroxyapatite/poly (vinyl alcohol) nanocomposites", Advances
in Applied Ceramics, 106, No.4, pp.165170.
27
[42] Karevan, M., Pucha, R.V., Bhuiyan, M.A., and Kalaitzidou, K., 2010, "Effect of
interphase modulus and nanofiller agglomeration on the tensile modulus of graphite
nanoplatelets and carbon nanotube reinforced polypropylene nanocomposites", Carbon
Letters, 11, No.4, pp.325331.
[43] Gonçalves, G., Marques, P.A., Barros, T.A., Bdkin, I., Singh, M.K., and Emami, N.,
2010, "Graphene oxide modified with PMMA via ATRP as a reinforcement filler",
Journal of Materials Chemistry, 20, No.44, pp.99279934.
[44] Gerstle, F.P., 1991, "Composites, In: Encyclopedia of Polymer Science and
Engineering", New York, NY: John Wiley & Sons.
[45] CST, "Fibers", http://www.cstsales.com.
[46] Abdulmajeed, A.A., Närhi, T.O., Vallittu, P.K., and Lassila, L.V., 2011, "The effect
of high fiber fraction on some mechanical properties of unidirectional glass fiber
reinforced composite", Dental Materials, 27, No.4, pp.313321.
[47] Akkapeddi, M., 2000, "Glass fiber reinforced polyamide‐6 nanocomposites",
Polymer Composites, 21, No.4, pp.576585.
[48] Iba, H., Chang, T., and Kagawa, Y., 2002, "Optically transparent continuous glass
fibrereinforced epoxy matrix composite: fabrication, optical and mechanical
properties", Composites Science and Technology, 62, No.15, pp.20432052.
[49] Iba, H., and Kagawa, Y., 1998, "Light transmittance of continuous fibrereinforced
composites: analysis, model experiment and parametric study", Philosophy Magazine B,
78, No.1, pp.3752.
[50] Lin, H., Kang, S.G., Day, D.E., and Stoffer, J.O., 1994, "The effect of fiber
annealing on the properties of an optically transparent PMMA composite", Composites
Science and Technology, 50, No.3, pp.367372.
[51] Kusano, Y., Norrman, K., Drews, J., Leipold, F., Singh, S.V., and Morgen, P., 2011,
"Gliding arc surface treatment of glassfiberreinforced polyester enhanced by ultrasonic
irradiation", Surface and Coatings Technology, 205, No.7, pp.490494.
[52] Ramesh, M., Palanikumar, K., and Hemachandra, R.K., 2012, "Mechanical property
evaluation of sisaljuteglass fiber reinforced polyester composites", Composites Part B:
Engineering, 48, No.5, pp.19.
[53] Rao, H.R., Rajulu, A.V., Reddy, G.R., and Reddy, K.H., 2010, "Flexural and
compressive properties of bamboo and glass fiberreinforced epoxy hybrid composites",
Journal of Reinforced Plastics and Composites, 29, No.10, pp.14461450.
28
[54] Manjunatha, C., Sprenger, S., Taylor, A., and Kinloch, A., 2010, "The tensile fatigue
behavior of a glassfiber reinforced plastic composite using a hybridtoughened epoxy
matrix", Journal of Composite Materials, 44, No.17, pp.20952109.
[55] Mazumdar, S., "Opportunities for thermoset resins in the composites industry",
http://www.trfa.org/erc/docretrieval/uploadedfiles/Technical%20Papers/2008%20Meetin
g/MazumdarLucintel_paperComposites_industry.pdf.
[56] Wikipedia, "Polyester", http://en.wikipedia.org/wiki/Polyester.
[57] Acmite Market Intellgence, "World epoxy resin market", http://www.acmite.
com/marketreports/chemicals/worldepoxyresinmarket.html.
[58] Kuo, C.C., 2012, "A simple and costeffective method for fabricating epoxybased
composite mold inserts", Materials and Manufacturing Processes, 27, No.4, pp.383388.
[59] Kim, J.K., Hu, C., Woo, R.S., and Sham, M.L., 2005, "Moisture barrier character
istics of organoclay–epoxy nanocomposites", Composites Science and Technology, 65,
No.5, pp.805813.
[60] Azom, "Resin properties for composite materials", http://www.azom.com/article.
aspx?ArticleID=997.
[61] Daeyang International Co. Ltd., http://www.alibaba.com/producttp/139744747/UPR
_191_196_Unsaturated_Polyester_Resin.html.
[62] Shanghai Shilei Chemical Co. Ltd., http://www.alibaba.com/product gs/555167436/
epoxy_resin.html.
[63] Dalian CR Science Development Co. Ltd., http://www.alibaba.com/productgs/
698902977/vinyl_ester_resin.html.
[64] Ji, F., Dharani, L., and Behr, R., 1998, "Damage probability in laminated glass
subjected to low velocity small missile impacts", Journal of Materials Science, 33, No.19,
pp.47754782.
[65] Kaiser, N.D., Behr, R.A., Minor, J.E., Dharani, L.R., Ji, F., and Kremer, P.A., 2000,
"Impact resistance of laminated glass using “sacrificial ply” design soncept", Journal of
Architecture Engineering, 6, No.1, pp.2434.
[66] Larcher, M., Solomos, G., Casadei, F., and Gebbeken, N., 2012, "Experimental and
numerical investigations of laminated glass subjected to blast loading", International
Journal of Impacting Engineering, 39, No.1, pp.4250.
29
[67] Lusk, B., Salim, H., Perry, K., Nawar, M., Wedding, W., and Kiger, S., 2011,
"Modeling and testing of laminated window systems under blast loading", Structures
Congress 2011: ASCE, pp.15521560.
[68] Türkmen, H., and Mecitoğlu, Z., 1999, "Dynamic response of a stiffened laminated
composite plate subjected to blast load", Journal of Sound Vibration, 221, No.3, pp.371
389.
[69] Wei, J., and Dharani, L., 2005, "Fracture mechanics of laminated glass subjected to
blast loading", Theory of Applied Fracture Mechanics, 44, No.2, pp.157167.
[70] Wei J., 2004, "Dynamics and failure analysis of architectural glazing subjected to
blast loading", Rolla, MO: University of Missouri.
[71] Amadio, C., and Bedon, C., 2012, "Blast analysis of laminated glass curtain walls
equipped by viscoelastic dissipative devices", Buildings, 2, No.3, pp.359383.
[72] Birman, V., and Bert, C.W., 1987, "Behaviour of laminated plates subjected to
conventional blast", International Journal of Impact Engineering, 6, No.3, pp.145155.
[73] Kazancı, Z., and Mecitoğlu, Z., 2008, "Nonlinear dynamic behavior of simply
supported laminated composite plates subjected to blast load", Journal of Sound
Vibration, 317, No.3, 883897.
30
CHAPTER 2 A NOVEL OPTICALLY TRANSPARENT
WOVEN GLASS FIBERREINFORCED POLYMER
COMPOSITE: FABRICATION AND PROPERTIES
2.1 Introduction
Transparent engineering polymers are needed in various fields, including aerospace,
military and automobile industries [1, 2]. Currently available transparent polymers have
some drawbacks, such as low quasistatic and dynamic mechanical properties.
Incorporation of glass fibers into a polymer matrix can greatly improve its mechanical
properties [36], while reducing its transparency (light transmittance) to some extent. The
transparency reduction is due to the refractive index mismatch between glass fibers and
the polymer matrix [3, 7]. Iba and Kagawa [8] studied the relationship between the
transparency and the refractive index difference and proposed an analytical model for
predicting the transparency of unidirectional aligned continuous fiberreinforced
composite. Based on Iba’s model, a new analytical model, which can be used to predict
the light transmittance of 0/90º woven glass fiberreinforced composite, has been
developed in this research.
Applications of optically transparent glass fiberreinforced polymer composite, such
as blast resistance screen and plane window, usually require high strength, good fracture
toughness and good dynamic impacting resistance [3, 913]. Hence, quasistatic
31
mechanical properties, fracture toughness and dynamic mechanical properties of a
transparent glass fiberreinforced composite should be investigated before using it.
Quasistatic mechanical properties and fracture toughness can be studied using an Instron
universal testing machine. Dynamic mechanical properties can be studied using a split
Hopkinson bar (SHB) [1420]. A series of SHB tests on glass fiberreinforced composite
have been performed previously [2125], reported results indicate that the dynamic
mechanical properties of glass fiberreinforced composite are dependent on strain rate.
In this study, an optically transparent woven (0/90º) glass fiberreinforced polyester
composite has been fabricated. The composite has been used as an interlayer in a blast
resistant laminated glass panel fabrication. A model for predicting the light transmittance
(transparency) of the composite has been proposed. According to the model, the light
transmittance can be increased by reducing the refractive index difference between glass
fibers and the polyester matrix. Since the refractive index of glass fibers is difficult to
change, the refractive index of the polyester matrix was modified to reduce the
difference. The modification was done by adjusting the concentrations of chemical
additives, such as methyl ethyl ketone peroxide (MEKP), cobalt (II) 2ethylhexanoate
(CE), divinylbenzene (DV) and phenanthrene (PT). Besides the refractive index
difference, the effect of fiber volume fraction on light transmittance was also studied.
Properties of the composite, such as quasistatic mechanical properties, fracture
toughness and dynamic mechanical properties, and viability of the fabricated laminated
glass under blast loading were investigated.
32
2.2 Experimental methods
2.2.1 Polyester plate fabrication
Polyester ((R’CH=CHCOOR)n, Ashland Specialty Co., USA) was mixed with 1.2
wt% methyl ethyl ketone peroxide (MEKP) (C8H18O6, SigmaAldrich Co., USA), an
initiator, 0.03 wt% cobalt (II) 2ethylhexanoate (CE) (C16H30CoO4, SigmaAldrich Co.,
USA), an accelerator and 4 wt% divinylbenzene (DV) (C10H10, SigmaAldrich Co., USA)
or 1 wt% phenanthrene (PT) (C14H10, SigmaAldrich Co., USA), which are refractive
index modifiers. All above mentioned components were thoroughly mixed for 34 min by
hand in a plastic bucket. The mixture was set in a vacuum degassing chamber so as to
allow air bubbles inside it to escape by creating vacuum inside the chamber. After
degassing, the mixture was poured into a 3.2 mm deep mold which was made by placing
aluminum frames on top of a polyvinyl chloride (PVC) plate with Mylar sheet (Fig. 2.1).
After filling the mold, another PVC plate with Mylar sheet was laid on top of the mold,
the top and bottom plates were clamped with Cclamps. The clamped plates were erected
sideways to let entrapped air escape from the mold. The setup was left at room
temperature (~20 ºC) for two days to ensure complete curing of the polyester.
33
Figure 2.1 Mold for fabricating polyester and glass fiberreinforced composite plates
2.2.2 Glass fiberreinforced composite fabrication
Glass fiberreinforced composite was prepared using a similar procedure as
described above. The polyester was mixed with 1.2 wt% MEKP, 0.03 wt% CE and 4
wt% DV or 1 wt% PT. All components were thoroughly mixed for 23 min by hand in a
plastic bucket. Then, the mixture was degassed in a vacuum chamber. But this time, after
degassing, instead of pouring all mixture into the 3.2 mm deep mold, a small amount of
the mixture was first poured into the mold so as to wet the base surface of the mold. Then
a layer of glass fiber cloth (Aerospace Composite Products Co., USA) was put in the
mold and some more polymer mixture was poured in the mold. This procedure was
repeated 4 times, producing a composite of 3.2 mm thick with 5 layers of glass fiber
34
cloth. The setup was left at room temperature for two days to ensure complete curing of
the composite. The cured composite had a fiber volume fraction of 12.3%.
Same procedure was also used to produce a composite of 1.6 mm thick with 5 layers
of glass fiber cloth. The cured composite had a fiber volume fraction of 24.2%.
The properties of glass fibers and polyester are listed in Table 2.1.
Table 2.1 Some properties of glass fibers and polyester
Glass fibers Polyester
Density (g/cm3)
Young’s modulus (GPa)
Poisson’s ratio
Refractive index at 589 nm at 20 ºC
Fiber diameter (μm)
Linear density* (fiber/mm)
2.54
70
0.2
1.5595
~10
~550
1.05
3.25
0.39



*transverse linear density and longitudinal linear density together.
2.2.3 Laminated glass panel fabrication
Laminated glass panel was fabricated by sandwiching the glass fiberreinforced
composite interlayer between two tempered glass sheets. The composite interlayer and
glass sheets were bonded using a two part polyurethane resin (SP&S Co., USA). The
procedure for fabricating a laminated glass is as follows: firstly, a glass sheet (Nashville
Tempered Glass Co., USA) was placed on a table and a very thin layer of polyurethane
resin was uniformly spread on the glass sheet. Secondly, the composite interlayer was
placed on top of the glass sheet. Pressure was applied to spread the resin and remove any
35
entrapped air bubbles. Finally, a very thin layer of polyurethane resin was uniformly
spread on the composite interlayer and the second glass sheet was placed on top of the
composite interlayer. The setup was left at room temperature for at least one day to
ensure complete curing of the polyurethane adhesive. The structure of the laminated glass
is shown in Fig. 2.2.
Figure 2.2 Laminated glass structure
2.2.4 Refractive index measurement
The refractive index of glass fibers (589 nm) was measured using the Central
Illumination Method (Becke Line Method).
Glass sheets
Composite
interlayer
Laminated glass
36
The refractive indices (589 nm) of polyester samples (25 mm × 8 mm ×3.2 mm)
were measured using Abbe refractometer (NAR3T, Atago Co., Japan, with a refractive
index precision of 0.0001 in the range of 1.3 to 1.7) at room temperature.
2.2.5 Light transmittance measurement
The light transmittance of the composite, polyester matrix and fabricated laminated
glass in the thickness direction was measured over a wavelength range of 190 to 900 nm
using an ultravioletvisible (UVVIS) spectrometer (UV 2401 PC, Shimadzu Co., Japan).
The resolution of the spectrometer is 1nm. All measurements were done at room
temperature.
2.2.6 Composite interlayer’s quasistatic mechanical properties testing
2.2.6.1 Young’s modulus and Poisson’s ratio
250 mm long and 25 mm wide strips were cut from the fabricated composite sheets
(Fig. 2.3). The strips were machined to ensure that they were straight and had smooth
edges. Aluminum tabs were attached to the gripped portions of the specimens to prevent
any possible damage (the shadow area in Fig. 2.3). Tensile tests were performed at room
temperature on a servohydraulic Instron 8800 universal testing machine with a 10 kN
load cell, at a crosshead speed of 2mm/min. For the measurement of tensile strains, strain
gages (CEA13240UZ120, Vishary Precision Inc., USA) were attached on the
specimens in both longitudinal (length direction) and lateral directions (width direction).
During the test, loads and strains were recorded by computer. These data were used to
37
find tensile strength T , failure strain f , Young’s modulus E and Poisson’s ratio v12.
ASTM D3039 [26] gives the following mathematical expression for calculating Young’s
modulus
(2.1)
P
bdE
where is the strain difference between two strain points in the initial linear region of
the stressstrain curve, P is the load difference between the same two points, b is the
specimen width, and d is the specimen thickness.
Poisson’s ratio 12 can be calculated using the following equation
12 = (2.2)la
lo
v
where la is the lateral strain difference between two lateral strain points and
lo is
the longitudinal strain difference between two corresponding longitudinal strain points.
25
mm
Aluminum tab
Strain
gageWire
Terminal
Wire connect to
Instron machine
Strain gage
Wire connect to
Instron machine
25 mm
250 mm
Figure 2.3 Shape and dimensions of tensile test specimens
38
2.2.6.2 Shear modulus
250 mm long and 25 mm wide ±45º fiberreinforced strips were cut from the
fabricated composite sheets. Strain gages were attached on the specimens in both
longitudinal and lateral directions. The ±45º specimens were loaded in tension while
recording loads and strains. According to the ASTM standard D3518 [27], shear modulus
G can be calculated as
= (2.3)G
where is the shear strain difference between two shear strain points. is the shear
stress difference between the same two shear strain points and is equal to 2P bd . P is
the load difference between the two shear strain points, b is the specimen width and d is
the specimen thickness.
2.2.7 Fracture toughness testing
The fracture toughness of the composite was investigated using Jintegral method. J
integral method is a way to calculate the work energy per unit fracture surface area of a
material. It has some advantages over the conventional stress intensity factor method,
such as its result evaluation is easier and its result is more accurate [28]. So in this study,
the Jintegral method was used to study the fracture toughness of the composite.
Jintegral method was developed by Cherepanov [29] and Jim Rice [30]
independently. The theoretical concept of the Jintegral method is that the energy integral
39
(called J) of a crack (notch) is independent of the path around it (Fig. 2.4). The Jintegral
value can be calculated using the following equation [30]
1
( , ) (2.4)1 2 2J W x x dx dsx
u
t
t σ n
where is a curve surrounding a crack (notch) tip. W(x1, x2) is the strain energy density,
x1, x2 are the coordinate directions, ds is the increment of the contour path, u is the
displacement vector, t is the surface traction vector, n is the vector normal to the curve
and σ is the Cauchy stress tensor. Landes and Begley [31] reported that at a constant
displacement, the Jintegral value for a specimen can be defined as
constant displacement
1= (2.5)
UJ
t a
where t is the thickness of the specimen, a is the crack length and U is the potential
energy.
40
notch
x1
x2
n
ds
Figure 2.4 Jintegral curve around a crack (notch)
In this research, Jintegral tests were carried out using singleedgenotchedtension
(SENT) specimens (Fig. 2.5) on the Instron 8800 universal testing machine with a 10 kN
load cell, at a crosshead speed of 2 mm/min. The dimensions of SENT specimens were
165 mm × 38 mm × 1.6 mm. Aluminum tabs were affixed to the gripped portions (the
shadow area in Fig. 2.5) of the specimens to prevent any possible damage. The total
length between grips was 115 mm. The cracks (notches) on the specimens were made by
first saw cutting and then sharpening with a diamond blade. The crack length (a) to
specimen width (w) ratio (a/w) was varied from 0.1 to 0.75 using the following discrete
ratios: 0.1, 0.15, 0.25, 0.35, 0.5, 0.6, 0.75. For every crack length, tests were conducted
on three specimens.
41
Figure 2.5 Dimensions of singleedgenotchedtension specimens
2.2.8 Dynamic mechanical properties testing
The dynamic mechanical properties of the composite were tested using the split
Hopkonson bar (SHB). Classical SHB system (Fig. 2.6 and 2.7) consists of two elastic
bars, called incident bar and transmitted bar, and a gas gun that can propel a striker bar.
The mechanism of SHB technique is: upon firing the gas gun, the striker bar imparts a
uniaxial stress pulse to the incident bar and a compressive stress wave generated in the
42
incident bar. This compressive stress wave travels in the incident bar and when this wave
reaches a specimen, part of it is reflected back to the incident bar and part of it is
transmitted through the specimen to the transmitted bar. The wave transmission in two
bars can be captured using strain gages placed on bars (Fig. 2.7). It should be pointed out
that before using SHB, it needs to be calibrated and the calibration procedures are
outlined in reference [32]. By analyzing the captured strain signals, the stress ( )s t ,
strain ( )s t and strain rate ( )s t of the specimen can be determined by the following
equations [33]
0
( ) (2.6)
2( ) (2.7)
2( ) (2.8)
s t
s
t
s r
s r
EAt t
A
ct t dt
L
ct t
L
where E is Young’s modulus of bars, A is the crosssectional area of bars, As is the cross
sectional area of the specimen, c is the stress wave velocity in bars, L is the length of the
specimen, ( )r t is the reflected strain signal and ( )t t is the transmitted strain signal.
43
Figure 2.6 Split Hopkinson bar (SHB) apparatus
Striker Bar
E, c, A
Incident Bar
εr
Specimen
(As)
εt Transmitted Bar
E, c, A
L
Strain gage Strain gage
Figure 2.7 Schematic of main components of a SHB system
44
Usually cylindrical specimens are used in SHB tests. But according to the results
reported by Woldesenbet et al. [34] and Phan [33], similar high strain rate mechanical
properties can be obtained by either using squareshape specimens or cylindricalshape
specimens. Since cylindrical specimens are relatively difficult to produce, square
specimens were used. The dimensions of test specimens were 6.4 mm × 6.4 mm × 3.2
mm
In this research, specimens were loaded in the thickness direction because in
dynamic applications, composite is usually loaded in the thickness direction. Fiber
orientation of specimens is 0/90º.
2.2.9 Fiber volume fraction determination
The fiber volume fraction of the composite was determined according to ASTM
D2584 [35]. A 25.4 mm × 25.4 mm × 1.6 mm composite specimen was weighed and
burnt in an empty ceramic crucible. Once the matrix resin was completely removed, the
residue was cooled to room temperature and weighted. The burnoff weight is the
polyester matrix weight and the residue weight is glass fibers weight. The fiber volume
fraction of the composite was calculated based on the following equation [36]
(2.9)m f
f
f m m f
WV
W W
where m and f are the density of the polyester matrix and glass fibers, respectively.
Wm is the matrix weight and Wf is fibers weight.
45
The fiber volume fraction of 3.2 mm thick composite was measured using the same
method.
2.2.10 Blast resistance testing
Blast resistance tests were done at the Engineering Research and Development
Center (ERDC, US Army Corps of Engineers Lab, Vicksburg, Mississippi) using a Blast
Load Simulator (BLS) (Fig. 2.8). The dimensions of the tested glass panels were 890 by
590 mm. The installation of a glass panel inside the BLS is shown in Fig. 2.9.
46
Figure 2.8 Blast Load Simulator (BLS)
Figure 2.9 Glass panel installation inside the BLS
47
2.3 Theoretical model for light transmission through woven glass fiber
reinforced composite
When light passes through a glass fiber, the phase of light beyond the fiber is
changed (Fig. 2.10). The maximum phase difference, which is also called the maximum
phase lag, can be expressed using equation (2.10) [8, 37]
2 (2.10)f f mδ= kr n  n
where fr is the radius of the glass fiber, k is the wavenumber of incident light and is
equal to 2 ( is the light wavelength), nf is the refractive index of the glass fiber, nm
is the refractive index of the surrounding matrix.
Figure 2.10 Phase of light after passing through a glass fiber
rfrfcosγ
γ
Fiber
Light
Phase of light after passing
through a glass fiber
Shadow
rfsinγ
48
The phase lag causes the reduction of the transmitted light intensity. The intensity
amplitude changes at a point at a distance of fr sinγ ( is the angle between the incident
light and surface of the glass fiber) from the center of the fiber is iδcosγe . Based on this,
the light transmittance T (ratio of transmitted light intensity to incident light intensity) of
a single fiberreinforced polymer composite can be expressed as [8]
2
01 2 1 (2.11)
2
π /iδcosγ
f m
f
f
s
T =  G Re  e cosγdγ T
rG =
w
where ws is the width of the composite, Gf is called shadow ratio and Tm is the light trans
mittance of the polymer matrix. Partial integration of equation (2.11) results in
222
0 0
22
0
1 2 1
1 2 (2.12)
π /π /
f m
π /
f m
T =  G sinγ  cos δcosγ +δ sin δcosγ sin γdγ T
=  G δ sin δcosγ sin γdγ T
From equation (2.12), it can be seen that light transmittance T increases with the decrease
of . Since 2 f f mδ= kr n  n , light transmittance T increases with the decrease of the
refractive index difference between the glass fiber and the polymer matrix.
For woven glass fiberreinforced polymer composite (0/90º woven fiber cloth, Fig.
2.11), the shadow ratio of one layer is: 2 2wf f t f lG = r ρ + r ρ , where t is the linear density
of fibers in the transverse direction, l is the linear density of fibers in the longitudinal
49
direction. Therefore, the light transmittance Tw of a composite with q layers of fiber cloth
can be calculated as
2
2
01 2 (2.13)
qπ /
w wf mT = G δ sin δcosγ sin γdγ T
From equation (2.13), it can be observed that for woven glass fiberreinforced composite,
the light transmittance Tw also increases with the decrease of phase lag . As mentioned
previously 2 f f mδ= kr n  n , so light transmittance Tw increases with the decrease of the
refractive index difference between glass fibers and the polymer matrix. In this research,
the refractive index of glass fibers was considered as fixed (1.5595). Therefore, in order
to increase the transparency of the glass fiberreinforced composite, the refractive index
of the polyester matrix was modified to reduce the refractive index difference between
glass fibers and the polyester matrix. The modification was done by changing the
concentrations of chemical additives in the polyester matrix.
50
Woven fiber
cloth
Light
Composite
ws
Transverse
direction
Longitudinal
direction
Figure 2.11 Light transmission model of woven glass fiberreinforced composite
From equation (2.13), it can also be observed that when the refractive index
difference is not zero, besides the refractive index difference, the light transmittance of
the composite also depends on the shadow ratio Gwf and the number of fiber layers q.
When the refractive index difference is zero ( =0 ), the light transmittance of the
composite is the same as that of the polyester matrix and in this situation, both the
shadow ratio Gwf and the number of fiber layers q can’t affect the light transmittance of
the composite. In this study, the shadow ratio Gwf is a constant value (constant fiber
radius, constant linear density in both longitudinal and transverse directions) and 5 layers
of fiber cloth were used to reinforce the polyester matrix. So the effects of the shadow
51
ratio Gwf and the number of fiber layers q on light transmittance are not discussed in this
study. It is worth pointing out that equation (2.13) does not explicitly incorporate the
effect of fiber volume fraction on light transmittance. But from this equation, it can be
inferred that the light transmittance of the composite can be affected by the change of
fiber volume fraction if the change affects the number of fiber layers the light encounters.
Otherwise, the light transmittance will not be affected by the change of fiber volume
fraction.
2.4 Results and discussion
2.4.1 Effects of chemical additives on the refractive index of polyester
2.4.1.1 Effect of methyl ethyl ketone peroxide (MEKP) concentration on
the refractive index of polyester
Fig. 2.12 shows the effect of MEKP concentration on the refractive index of
polyester. With the increase of MEKP concentration, the refractive index of polyester
varies around 1.5560. Increasing MEKP concentration has almost no effect on the
refractive index of polyester.
52
Figure 2.12 Refractive index of polyester (cured product) with different MEKP concentrations
(curing condition: curing temperature 20 ºC, CE 0.03 wt%)
2.4.1.2 Effect of cobalt (II) 2ethylhexanoate (CE) concentration on the
refractive index of polyester
From Fig. 2.13, it can be seen that the refractive index of polyester increases with
the increase of CE concentration. CE is used as the polymerization accelerator in this
study and its color is reddish violet. More CE content in polyester means smaller gel
time, less curing time and deeper color in the cured product. According to experimental
0 0.5 1 1.5 2 2.51.554
1.5545
1.555
1.5555
1.556
1.5565
1.557
1.5575
1.558
MEKP concentration (wt%)
Ref
ract
ive
index
of
poly
este
r (c
ure
d p
roduct
)
53
results, when CE concentration is more than 0.04 wt%, polyester cures very fast and
cured product has a dark amber color. When CE concentration is less than 0.01 wt%,
polyester cures very slowly. Therefore, appropriate CE concentration should be between
0.01 wt% and 0.04 wt%.
Figure 2.13 Refractive index of polyester (cured product) with different CE concentrations
(curing condition: curing temperature 20 ºC, MEKP 1.2 wt%)
0.01 0.02 0.03 0.04 0.05 0.06 0.071.55
1.555
1.56
1.565
CE concentration (wt%)
Ref
ract
ive
index
of
poly
este
r (c
ure
d p
roduct
)
54
2.4.1.3 Effect of divinylbenzene (DV) concentration on the refractive
index of polyester
Fig. 2.14 illustrates the effect of DV concentration on the refractive index of
polyester. It can be seen that the refractive index of polyester increases with the increase
of DV concentration. The reason for this phenomenon is that besides as a refractive index
modifier, DV is also a crosslinker, with the increase of DV concentration, the
crosslinking density of polyester increases which results in the increase of refractive
index. Similar reports have been reported by Askadskii [38] and Murakami [39] that
refractive indices of polymers can be increased by increasing the crosslinking density of
polymers. When DV concentration is 3 wt%, the refractive index of polyester is 1.5581.
When DV concentration is 10 wt%, the refractive index of polyester is 1.5624, which is
much higher than that of glass fibers which is 1.5595. So, appropriate DV concentration
is between 3 wt% and 7 wt%.
55
Figure 2.14 Refractive index of polyester (cured product) with different DV concentrations
(curing condition: curing temperature 20 ºC, CE content 0.03 wt%, MEKP 1.2 wt%)
2.4.1.4 Effect of phenanthrene (PT) concentration on the refractive
index of polyester
From Fig. 2.15, it can be seen that the refractive index of polyester increases
dramatically as PT concentration increases from 0 wt% to 1.2 wt% and increases slowly
with further increase in PT concentration. PT is a chemical with high refractive index
(1.5943) and is used as a refractive index modifier in this research. When PT content is 0
wt%, the refractive index of polyester is 1.5560. When PT content is 1.2 wt%, the
0 5 10 15 20 251.555
1.56
1.565
1.57
DV concentration (wt%)
Ref
ract
ive
index
of
poly
este
r (c
ure
d p
roduct
)
56
refractive index of polyester is 1.5608. Therefore, appropriate PT concentration is
between 0 wt% and 1.2 wt%.
Figure 2.15 Refractive index of polyester (cured product) with different PT concentrations
(curing condition: curing temperature 20 ºC, CE content 0.03 wt%, MEKP 1.2 wt%)
According to experimental results, two candidate formulations for making the
transparent glass fiberreinforced polymer composite are listed in Table 2.2. The second
formulation is not recommended. Because PT is solid at room temperature, after curing,
undissolved PT particles are left in the cured composite, which affects the transparency of
the composite. This problem does not apply to the first formulation because DV is liquid
0 0.5 1 1.5 2 2.5 31.555
1.556
1.557
1.558
1.559
1.56
1.561
1.562
PT concentration (wt%)
Ref
ract
ive
index
of
poly
este
(cu
red p
roduct
)
57
at room temperature. Therefore, the best formulation for making the optically transparent
glass fiberreinforced composite is: MEKP concentration=1.2 wt%, DV concentration=4
wt% and CE concentration=0.03 wt%.
Table 2.2 Candidate formulations for making the optically transparent composite
MEKP
concentration
DV concentration PT concentration CE
concentration
Refractive
index
1
2
1.2 wt%
1.2 wt%
4 wt%
0 wt%
0 wt%
1 wt%
0.03 wt%
0.03 wt%
1.5587
1.5599
2.4.2 Light transmittance
2.4.2.1 Light transmittance of the composite interlayer
Fig. 2.16 shows the light transmittance spectrum of the polyester matrix. The
spectrum shows that above a wavelength of 380 nm, the light transmittance of the
polyester matrix first dramatically increases to 77.5%, then slowly increases to 86.7%.
Fig. 2.16 also shows the light transmittance spectra of the composite specimens
prepared using the best formulation (1.6 mm thick composite specimen with a fiber
volume fraction of 24.2% and 3.2 mm thick composite specimen with a fiber volume
fraction of 12.3%, both have 5 layers of fiber cloth). With the increase of light
wavelength, the light transmittance of the 3.2 mm thick composite specimen first
increases to 74.5%, then decreases to 65%. The light transmittance spectrum of the 1.6
mm thick composite specimen is almost the same as that of the 3.2 mm thick composite
specimen. This verifies the inference derived from the theoretical analysis that the light
58
transmittance of the composite will not be affected by the change of fiber volume fraction
if the change does not affect the number of fiber layers the light encounters.
Figure 2.16 Comparison between experimentally measured light transmittance and
theoretically predicted light transmittance
The light transmittance of the composite with 5 layers of fiber cloth is predicted
using equation (2.13) and plotted in Fig. 2.16. It can be observed that at a wavelength of
589 nm, the theoretically calculated light transmittance coincides with the experimentally
measured light transmittance of the 3.2 mm thick composite specimen and almost
coincides with the light transmittance of the 1.6 mm thick composite specimen. Beyond
100 200 300 400 500 600 700 800 9000
10
20
30
40
50
60
70
80
90
100
Wavelength (nm)
Tra
nsm
itta
nce
(%
)
Light transmittance of 1.6 mmthick composite
Light transmittance of3.2 mm thick composite
Light transmittance of pure polyester
Theoretically predictedlight transmittance
59
or below this wavelength, the theoretically calculated light transmittance curve strays
from the experimentally measured light transmittance curves. The difference between the
calculated result and the measured results is due to the wavelength dependence of
refractive index [40]. In this study, all measured refractive indices are the refractive
indices at 589 nm. Therefore at 589 nm, the refractive index difference between glass
fibers and the polyester matrix is the ‘real refractive index difference’. Equation (2.13)
can effectively predict the light transmittance at this wavelength. Beyond or below this
wavelength, because of the wavelength dependence of refractive index, the refractive
indices of the polyester matrix and glass fibers both change which means the refractive
index difference between them is different from the difference at 589 nm. So, except 589
nm, at other wavelengths, equation (2.13) use ‘fake’ refractive index difference
(refractive index difference at 589 nm) to predict the light transmittance which results in
the mismatch of the theoretically predicted result and the experimentally measured results.
If the relationship between refractive index and wavelength of glass fibers and the
polyester matrix can be obtained, the light transmittance over the whole spectrum could
be predicted more precisely by the developed model.
The appearance of the glass fiberreinforced composite prepared using the best
formulation (3.2 mm thick, the appearance of the 1.6 mm thick composite is similar) and
the polyester matrix is shown in Fig. 2.17. Characters underneath the composite plate and
the polyester plate can be clearly read, indicating that the composite and the polyester
matrix are both optically transparent.
60
Figure 2.17 Readability of text through the glass fiberreinforced composite plate and the polyester plate
Besides the light wavelength, temperature may also cause the change of the
refractive index difference since the polyester matrix and glass fibers have different
refractive indextemperature relations. The composite plate shown above was heated to
60 ºC (the maximum expected using temperature) for 3 h and no transparency change
was noticed, which indicates that in this study, the effect of temperature on the
transparency can be neglected.
2.4.2.2 Light transmittance of the laminated glass
Fig. 2.18 shows the light transmittance of the laminated glass utilizing the glass
fiberreinforced composite interlayer over a wavelength range of 190 to 900 nm. The
light transmittance of the laminated glass is above 60% when the wavelength is above
482 nm. The highest transmittance is 84.4% when the wavelength is 577 nm. This result
Polyester plate
Glass fiberreinforced
composite
61
means the fabricated laminated glass has good transparency in the visible light range. The
good transparency is achieved by using the transparent composite interlayer.
Appearance of the laminated glass is shown in Fig. 2.19. Through the laminated
glass, the backside view can be clearly observed, which shows the fabricated laminated
glass has good transparency. This result coincides with the light transmittance spectrum
analysis result shown above.
Figure 2.18 Light transmittance spectrum of the laminated glass
100 200 300 400 500 600 700 800 9000
10
20
30
40
50
60
70
80
90
Wavelength (nm)
Tra
nsm
itta
nce
(%
)
62
Figure 2.19 Appearance of the fabricated laminated glass
2.4.3 Quasistatic mechanical properties
The longitudinal stressstrain curves of the glass fiberreinforced composite
specimens (1.6 mm thick composite and 3.2 mm thick composite) are shown in Fig. 2.20,
Young’s modulus of the composite specimens is calculated using equation (2.1). The
value of 3.2 mm thick composite is 7.67 GPa and the value of 1.6 mm thick composite is
12.33 GPa, which are both much higher than that of the neat polyester (~3 GPa) [41]. The
initial linear parts of the stressstrain curves are plotted in Fig. 2.21 and the corresponding
lateral stressstrain curves in the same region are also plotted in Fig. 2.21. Poisson’s ratio
v12 of the composite, which is 0.33 for 3.2 mm thick composite and 0.39 for 1.6 mm thick
composite, is found by using equation (2.2) and Fig. 2.21. The shear stressstrain curves
of the composite specimens in the initial loading range are plotted in Fig. 2.22. The shear
63
modulus of the composite is calculated using equation (2.3). For 3.2 mm thick composite,
shear modulus is 2.14 GPa and for 1.6 mm thick composite, shear modulus is 3.39 GPa.
Figure 2.20 Stressstrain curves of the glass fiberreinforced composites
0 0.002 0.004 0.006 0.008 0.01 0.012 0.0140
50
100
150
Strain (m/m)
Str
ess
(MP
a)
Fiberreinforced composite(3.2 mm)
Fiberreinforcedcomposite (1.6 mm)
64
Figure 2.21 Stress vs. strain curves of the composites in the initial linear region
Figure 2.22 Shear stressstrain curves of the glass fiberreinforced composites
4 2 2 4 6 8
20
40
60
80
100
Strain (m/m)
Str
ess
(MP
a)
x 103
Lateral stressstraincurve (1.6 mm)
Longitudinal stressstraincurve (3.2 mm)
Lateral stressstraincurve (3.2 mm)
Longitudinal stressstraincurve (1.6 mm)
0 0.5 1 1.5 2 2.5
x 103
0
1
2
3
4
5
6
7
8
Shear strain (, m/m)
Sh
ear
stre
ss ( ,
MP
a)
Fiberreinforced composite(1.6 mm)
Fiberreinforced composite(3.2 mm)
65
All quasistatic mechanical properties of the composites are listed in Table 2.3.
Table 2.3 Quasistatic mechanical properties of the glass fiberreinforced composites
Tensile strength
(σT, MPa)
Failure strain
(εf)
Young’s modulus
(E, GPa)
Poisson’s
ratio (v12)
Shear modulus
( , GPa)
Fiberreinforced
composite (3.2
mm thick, fiber
volume fraction
12.3%)
Fiberreinforced
composite (1.6
mm thick, fiber
volume fraction
24.2%
Polyester
PVB
41.95
139.9
21.65
0.0082
0.0125
0.0064
7.67
12.33
3.25
~0.1
0.33
0.39
0.448
2.14
3.39
2.4.4 Fracture toughness
The loaddisplacement curves for 0/90º woven glass fiberreinforced composite
specimens with different initial crack lengths are shown in Fig. 2.23. From Fig. 2.23, it
can be seen that for specimens with small cracks, fracture causes a sharp drop in load
after the maximum load; for specimens with large cracks, fracture causes a gradual drop
in load after the maximum load. The reason for this phenomenon is that the strain energy
stored in specimens with small cracks is sufficient to cause sudden failure [42]. It is not
the case for specimens with large cracks.
From Fig. 2.23, it can also be seen that the maximum carrying load of the composite
decreases with the increase of initial crack length. The displacement at maximum load
(critical displacement) decreases as initial crack length increases from 3.8 to 13.3 mm
and remains nearly constant at 0.9 mm with further increase in initial crack length. The
66
reason for this phenomenon is that when initial crack length is longer than the critical
initial crack length (13.3 mm), the fracture behavior of the composite is mainly governed
by the initial crack so that the critical displacement is nearly constant. When initial crack
length is less than 13.3 mm, the fracture behavior of the composite is influenced not only
by the initial crack, but also by elastic and plastic deformations away from the crack
plane [28]. Therefore, the critical displacement is not constant in this crack length region.
It increases with the decrease of initial crack length.
Figure 2.23 Loaddisplacement curves for fiberreinforced composite specimens with different initial crack
lengths (a is crack length and w is specimen’s width)
The loaddisplacement curves shown in Fig. 2.23 are used to calculate the potential
energy U in equation (2.5). It should be pointed out that when displacement is constant,
0 0.2 0.4 0.6 0.8 1 1.2 1.40
500
1000
1500
2000
2500
3000
3500
4000
4500
Displacement(mm)
Lo
ad(N
)
a = 3.8mm(a/w = 0.1)
a = 5.7 mm (a/w = 0.15)
a = 9.5 mm(a/w = 0.25)
a = 13.3 mm(a/w = 0.35)
a = 19 mm(a/w = 0.5)
a = 22.9 mm(a/w = 0.6)
a = 28.5 mm(a/w = 0.75)
67
the potential energy U is equal to the strain energy which can be obtained by measuring
the area under the loaddisplacement curve [31]. In order to obtain the Jintegral value at
different displacements, six displacements (0.18 mm, 0.36 mm, 0.54 mm, 0.72 mm, 0.90
mm and 0.95 mm) are chosen. For each displacement, the area under the load
displacement curves are measured, divided by thickness (B) and plotted against initial
crack lengths (Fig. 2.24).
From Fig. 2.24, it can be seen that for a given displacement, the strain energy per
unit thickness of the glass fiberreinforced composite decreases as initial crack length
increases, because the specimen with larger initial crack length has smaller loadcarrying
ability. For each displacement, variation of strain energy per unit thickness with initial
crack length can be represented by two straight lines. Two lines intersect at a crack length
of 13.3 mm, which shows a change in fracture behavior at this crack length. This result
corresponds to the result observed in Fig. 2.23, which shows the fracture behavior of the
composite changes at the crack length of 13.3 mm. Jintegral values are obtained by
calculating the slopes of the lines shown in Fig. 2.24. Based on the initial crack length
(a/w ≥ 0.35 or a/w < 0.35), two Jintegral value versus displacement curves are obtained
and plotted in Fig. 2.25. From Fig. 2.25, it can be seen that the Jintegral value at the
critical displacement, referred to as the critical value of Jintegral (Jc), is 22.1 kJ/m2 when
a/w ≥ 0.35. When a/w < 0.35, Jc can’t be evaluated directly through Fig. 2.25 since the
corresponding Jintegral curve does not reach the critical displacements in this range.
According to the reference [28], the Jc value for small initial crack length (here is a/w <
68
0.35) is close to the Jc value for large crack length (here is a/w ≥ 0.35) . Therefore, in this
research, the Jc value of glass fiberreinforced composite is determined as 22.1 kJ/m2.
Figure 2.24 Strain energy per unit thickness versus initial crack length at different displacements
0 5 10 15 20 25 300
100
200
300
400
500
600
700
800
900
Crack length (mm)
Str
ain
en
erg
y p
er u
nit
th
ick
nes
s (J
/m)
Crack length is 3.8 mm
Crack length is 5.7 mm
Crack length is 9.5 mm
Crack length is 13.3 mm
Crack length is 19 mm
Crack length is 22.9 mm
Crack length is 28.5 mm
0.95 mm(Displacement)
0.9mm
0.54mm
0.72mm
0.36mm
0.18mm
69
Figure 2.25 Jintegral curves of the composite
2.4.5 Dynamic mechanical properties
The strain rate range studied in this research is approximately between 4001000 s1
,
which is typical strain rate range for blast loading. Within this strain rate range, the valid
experimental results should satisfy two required conditions of SHB test. These conditions
are 1) achievement of constant strain rate and 2) achievement of stress equilibrium for
duration of the incident pulse.
The effect of strain rate on the dynamic mechanical properties of the glass fiber
reinforced composite is presented in Fig. 2.26. It clearly shows that the dynamic stress
0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 10
5
10
15
20
25
Displacement (mm)
Jin
teg
ral
(kJ/
m2)
Jc = 22.1 kJ/m2
a/w 0.35
a/w < 0.35
70
strain curve of the composite is affected by strain rate. At different strain rates, the
compressive modulus and compressive strength values of the composite are listed in
Table 2.4. The compressive modulus presented in this article should be regarded as the
approximate compressive modulus since there is an unavoidable uncertainty in
determining the compressive modulus by using the SHB technique [16, 43]. From Table
2.4, it can be seen that the compressive modulus of the composite increases as strain rate
increases. Also, it can be seen that the compressive strength of the composite increases as
strain rate increases (Fig. 2.27). The compressive strength increases by about 25% as
strain rate increasing from 407 s1
to 960 s1
. Similar trends have been reported by Li et
al. [44] and Kim et al. [16]. This phenomenon may be caused by the decrease of polymer
chains’ molecular mobility with the increase of strain rate [45, 46]. A linear equation
(2.14) is used to characterize the rate dependence of the compressive strength. The linear
relationship is
=0.099* +174.15 (2.14)cσ
where cσ is the compressive strength, is the strain rate. The limitation of this
relationship is that it is only applicable to the strain rate between 400 and 1000 s1
.
71
Figure 2.26 Stressstrain curves of the glass fiberreinforced composite at different strain rates
Table 2.4 Dynamic mechanical properties of the glass fiberreinforced composite
Strain rate (s1
) Compressive modulus (GPa) Compressive strength (MPa)
407
657
802
960
9.29
11.01
11.21
12.02
218.32
233.27
253.46
271.03
0 0.02 0.04 0.06 0.08 0.1 0.12 0.140
50
100
150
200
250
300
Strain (m/m)
Str
ess
(MP
a)
407 s1
657 s1
802 s1
960 s1
72
Figure 2.27 Effect of strain rate on compressive strength of the glass fiberreinforced composite
After SHB tests, the fracture morphology of the composite was examined using an
Olympus optical microscope (BX41MLED, Olympus Co., Japan) (Fig. 2.28). When
strain rate is 407 s1
, there are no clearly visible cracks on the impact surface of the
composite (Fig. 2.28 (a)). When strain rate is 657 s1
, some fiber lines can be clearly
observed on the surface, which means fibers begin to delaminate from the polyester
matrix (Fig. 2.28 (b)). When strain rate is 802 s1
, cracks can be observed on the surface
(Fig. 2.28 (c)). When strain rate is 960 s1
, a network of cracks appears on the surface
((Fig. 2.28 (d)). So, the impactintroduced failure process of the composite is as follows:
200 300 400 500 600 700 800 900 1000 1100 1200210
220
230
240
250
260
270
280
Strain rate (s1
)
Str
ess
(MP
a)
.
c=0.099*+174.5
73
with the increase of strain rate, fibers first delaminate from the polyester matrix as a
consequence of fiber/matrix interfacial debonding. Then, on further increase in strain
rate, the delamination grows continuously, surface cracks tend to appear and propagate
into the matrix. Specimens tested with strain rates higher than 1000 s1
broke into pieces
during the test.
(a) (b)
(c) (d)
Figure 2.28 Surface micrographs of the glass fiberreinforced composite at different strain rates:
(a) 407 s1
; (b) 657 s1
; (c) 802 s1
; (d) 960 s1
2.4.6 Blast resistance testing results
U.S. General Services Administration (GSA) blast loading levels C, D and E were
used for tests done at ERDC. Level C specifies a minimum peak pressure of 4 psi (25.8
100 µm 100 µm
100 µm
100 µm
100 µm
100 µm
100 µm
74
kPa) and impulse of 28 psimsec (193 kPamsec), while level D specifies a minimum
peak pressure of 10 psi (69 kPa) and impulse of 89 psimsec (614 kPamsec). Level E is
not specifically quantified by GSA but for this study we assumed level E as peak pressure
greater than 20 psi (138 kPa) and impulse greater than 115 psimsec (793 kPamsec).
Laminated window panels were tested under different blast loading levels. Window
panels of 3/8 inch (9.5 mm) total thickness consisting of a 1/8 inch (3.2 mm) thick
transparent composite interlayer laminated to two 1/8 inch (3.2 mm) thick tempered glass
sheets were tested under level C and D with no damage to the windows. The same
window construction as above but with a total thickness of 7/16 inch (11.1 mm), due to
use of 1 mm thick urethane based adhesive layer on each side of the interlayer, was tested
at level E, which resulted in cracks in the glass glazing with no fallout of glass and
minimal damage to the composite interlayer, as shown in Fig. 2.29. A 3/8 inch thick
window panel was tested under a blast condition over the minimum specified level E,
which resulted in extensive damage to the window panel and it was partially dislodged
from the frame as shown in Fig. 2.30. A thicker window of 5/8 inch (16 mm) total
thickness consisting of two composite interlayers laminated to three glass layers (each 1/8
inch or 3.2 mm thick) was tested under blast loading well over the minimum specified
level E, which resulted in cracking of the frontal and rear glass layers with no apparent
damage to the composite interlayers or any fallout of glass, as seen in Fig. 2.31. The
above mentioned blast testing demonstrates the viability of the novel glass window panel
utilizing a transparent fiberreinforced polymer composite interlayer under high intensity
blast loading.
75
Field experiments are expensive and timeconsuming. In order to save money and
time, a numerical model is developed to predict the dynamic response of the laminated
glass panel under different blast loading conditions. This model will be presented in the
next chapter.
Figure 2.29 Laminated glass window panel was cracked after the GSA level E blast test. Both the outer
surfaces of the glass plies were smooth to touch and minor damage to the composite interlayer
76
Figure 2.30 Level E blast loading resulted in severe damage to the window panel
Figure 2.31 Thicker glass window panel after Level E blast loading
77
2.5 Summary
An optically transparent woven glass fiberreinforced polyester matrix composite
has been successfully fabricated and utilized as an interlayer in a laminated glass panel.
The properties of the composite interlayer and the laminated glass were studied. The
main findings that can be inferred are as follows:
(1) A theoretical model for predicting the light transmittance of woven glass fiber
reinforced composite has been proposed. Theoretical analysis shows the transparency of
the glass fiberreinforced composite can be improved by reducing the refractive index
difference between glass fibers and its matrix. In this research, the refractive index of
glass fibers was considered as fixed. So the refractive index difference was minimized by
chemically changing the refractive index of the polyester matrix. Effects of MEKP, CE,
DV and PT concentrations on the refractive index of the polyester matrix were
investigated. The best formulation for making an optically transparent composite is:
MEKP concentration=1.2 wt%, DV concentration=4 wt% and CE concentration=0.03
wt%.
(2) The theoretical model also shows that besides the refractive index difference, the
transparency of the glass fiberreinforced composite also depends on the number of fiber
layers the incident light encounters. This inference has been verified by experimental
results.
(3) The light transmittance spectra and appearance of the composite prepared using
the best formulation and the corresponding laminated glass indicate the developed glass
78
fiberreinforced polymer composite and the laminated glass both have good transparency
in the visible light region.
(4) Quasistatic test results show that the glass fiberreinforced composite has much
better mechanical properties than the polyester matrix.
(5) The fracture toughness of the composite based on the Jintegral method is Jc=
22.1 kJ/m2.
(6) Split Hopkinson bar test results show that the dynamic mechanical properties of
the composite are strain rate sensitive. Compressive modulus and compressive strength
both increase with the increase of strain rate over the range 4001000 s1
.
(7) Blast loading tests done at ERDC show the new laminated glass panels perform
well under GSA specified C, D and E blast loading levels. This demonstrates the viability
of the new laminated glass window panel under high intensity blast loading.
79
REFERENCES
[1] O’Brien, D.J., and Parquette, B., 2012, "Polymer toughness transfer in a transparent
interpenetrating glass–polymer composite", Composites Science and Technology, 73,
pp.5763.
[2] Brennan, R.E., and Green, W.H., 2011, "Nondestructive characterization of low
velocity impact damage in transparent laminate systems", Hoboken, NJ: John Wiley &
Sons.
[3] Iba, H., Chang, T., and Kagawa, Y., 2002, "Optically transparent continuous glass
fibrereinforced epoxy matrix composite: fabrication, optical and mechanical
properties", Composites Science and Technology, 62, No.15, pp.20432052.
[4] Olson, J.R., Day, D.E., and Stoffer, J.O., 1992, "Fabrication and mechanical
properties of an optically transparent glass fiber/polymer matrix composite", Journal of
Composite Materials, 26, No.8, pp.11811192.
[5] Novak, B.M., 1993, "Hybrid nanocomposite materials—between inorganic glasses
and organic polymers", Advanced Materials, 5, No.6, pp.422433.
[6] Moriwaki, T., 1996, "Mechanical property enhancement of glass fibrereinforced
polyamide composite made by direct injection moulding process", Composites Part A:
Applied Science and Manufacturing, 27, No.5, pp.379384.
[7] Iba, H., Naganuma, T., Matsumura, K., and Kagawa, Y., 1999, "Fabrication of
transparent continuous oxynitride glass fiberreinforced glass matrix composite", Journal
of Materials Science, 34, No.23, pp.57015705.
[8] Iba, H., and Kagawa, Y., 1998, "Light transmittance of continuous fibrereinforced
composites: analysis, model experiment and parametric study", Philosophical Magazine
Part B, 78, No.1, pp.3752.
[9] Sarva, S., Mulliken, A.D., Boyce, M.C., and Hsieh, A.J., 2004, "Mechanics of
transparent polymeric material assemblies under projectile impact: simulations and
experiments", DTIC Document.
[10] Yahya, M.Y., Cantwell, W.J., Langdon, G., and Nurick, G., 2008, "The blast
behavior of fiber reinforced thermoplastic laminates", Journal of Composite Materials,
42, No.21, pp.22752297.
[11] Avci, A., Arikan, H., and Akdemir, A., 2004, "Fracture behavior of glass fiber
reinforced polymer composite", Cement and Concrete Research, 34, No.3, pp.429434.
80
[12] Nikpur, K., Chen, Y., and Kardos, J., 1990, "Fracture toughness of unidirectional
shortfiber reinforced epoxy composites", Composites Science and Technology, 38, No.2,
pp.175191.
[13] Mouritz, A., 2001, "Ballistic impact and explosive blast resistance of stitched
composites", Composites Part B: Engineering, 32, No.5, pp.431439.
[14] Pankow, M., Salvi, A., Waas, A., Yen, C., and Ghiorse, S., 2011, "Split Hopkinson
pressure bar testing of 3D woven composites", Composites Science and Technology, 71,
No.9, pp.11961208.
[15] Hokka, M., Kuokkala, V.T., and Ihme, S., 2009, "Dynamic tensile testing of
polyamide sheets using the HSB technique", Proceedings of the 2009 SEM Annual
Conference and Exposition on Experimental and Applied Mechanics, pp.17.
[16] Kim, W., Argento, A., Lee, E., Flanigan, C., Houston, D., and Harris, A., 2012,
"High strainrate behavior of natural fiberreinforced polymer composites", Journal of
Composite Materials, 46, No.9, pp.10511065.
[17] Jiang, F., and Vecchio, K.S., 2009, "Hopkinson bar loaded fracture experimental
technique: a critical review of dynamic fracture toughness tests", Applied Mechanics
Reviews, 62, No.6, pp.139.
[18] Tekalur, S.A., Shukla, A., and Shivakumar, K., 2008, "Blast resistance of polyurea
based layered composite materials", Composite Structures, 84, No.3, pp.271281.
[19] Hosur, M., Alexander, J., Jeelani, S., Vaidya, U., and Mayer, A., 2003, "High strain
compression response of affordable woven carbon/epoxy composites", Journal of
Reinforced Plastics and Composites, 22, No.3, pp.271296.
[20] Hosur, M., Alexander, J., Vaidya, U., Jeelani, S., and Mayer, A., "Studies on the off
axis high strain rate compression loading of satin weave carbon/epoxy composites",
Composite Structures, 63, No.1, pp.7585.
[21] Shokrieh, M.M., and Omidi, M.J., 2009, "Compressive response of glass–fiber
reinforced polymeric composites to increasing compressive strain rates", Composite
Structures, 89, No.4, pp.517523.
[22] Cao, M.S., Song, W.L., Zhou, W., Wang, D.W., Rong, J.L., and Yuan, J., 2010,
"Dynamic compressive response and failure behavior of fiber polymer composites
embedded with tetraneedlelike ZnO nanowhiskers", Composite Structures, 92, No.12,
pp.29842991.
[23] Shokrieh, M.M., and Omidi, M.J., 2009, "Tension behavior of unidirectional
glass/epoxy composites under different strain rates", Composite Structures, 88, No.4,
pp.595601.
81
[24] Schoßig, M., Bierögel, C., Grellmann, W., and Mecklenburg, T., 2008, "Mechanical
behavior of glassfiber reinforced thermoplastic materials under high strain rates",
Polymer Testing, 27, No.7, pp.893900.
[25] Song, B., Chen, W., and Weerasooriya, T., 2003, "Quasistatic and dynamic
compressive behaviors of a S2 glass/SC15 composite", Journal of Composite Materials,
37, No.19, pp.17231743.
[26] ASTM, "Standard test method for tensile properties of polymer matrix composite
materials", West Conshohocken, PA: ASTM International.
[27] ASTM, "Standard test method for inplane shear response of polymer matrix
composite materials by tensile test of a ±45° laminate", West Conshohocken, PA: ASTM
International.
[28] Agarwal, B., Kumar, P., and Khanna, S.K., 1986, "Determination of the fracture
toughness of fabric reinforced composites by the Jintegral approach", Composites
Science and Technology, 25, No.4, pp.311323.
[29] Cherepanov, G., 1967, "Crack propagation in continuous media PMM",
Journal of Applied Mathematics and Mechanics, 31, No.3, pp.503512.
[30] Rice, J.R., 1967, "A path independent integral and the approximate analysis of
strain concentration by notches and cracks", Journal of Applied Mechanics, 35, No.2,
379386.
[31] Landes, J., and Begley, J., 1972, "The effect of specimen geometry on J/c. fracture
toughness", Proceedings of the 1971 National Symposium on Fracture Mechanics, pp.24
39.
[32] Gama, B.A., Lopatnikov, S.L., and Gillespie, J.W., 2004, "Hopkinson bar
experimental technique: A critical review", Applied Mechanics Reviews, 57, No.4,
pp.223250.
[33] Phan, H.T., 2012, "High strain rate behavior of graphene reinforced polyurethane
composites", Columbia, MO: University of Missouri.
[34] Woldesenbet, E., and Vinson, J.R., 1999, "Specimen geometry effects on highstrain
rate testing of graphite/epoxy composites", AIAA Journal, 37, No.9, pp.11021106.
[35] ASTM, "Standard test method for ignition loss of cured reinforced resins", West
Conshohocken, PA: ASTM International.
[36] Aditi, C., 2012, "Onorbit assessment of satellite structural properties via robust
structural health monitoring", Tempe, AZ: Arizona State University.
82
[37] Van, D.H.H.C., 1981, "Light scattering by small particles", Mineola, NY: Dover
Publications.
[38] Askadskii, A.A., 1990, "Influence of crosslinking density on the properties of
polymer networks", Polymer Science USSR, 32, No.10, pp.20612069.
[39] Murakami, K., and Ando, S., 2011, "Effects of UV crosslinking under high
temperature on the refractive indices and aggregation structures of benzophenone
containing polyimides", Journal of Photopolymer Science and Technology, 24, No.3,
pp.277282.
[40] Jenkins, F.A., and White, H.E., 1957, 3rd ed., "Fundamentals of optics", New York,
NY: McGrawHill.
[41] Pothan, L.A., Mai, Y., Thomas, S., and Li, R., 2008, "Tensile and flexural behavior
of sisal fabric/polyester textile composites prepared by resin transfer molding technique",
Journal of Reinforced Plastics and Composites, 27, No.1617, pp.18471866.
[42] Agarwal, B.D., Patro, B.S., and Kumar, P., 1984, "J integral as fracture criterion for
short fibre composites: An experimental approach", Engineering Fracture Mechanics, 19,
No.4, pp.675684.
[43] AlMousawi, M., Reid, S., and Deans, W., 1997, "The use of the split Hopkinson
pressure bar techniques in high strain rate materials testing", Proceedings of the
Institution of Mechanical Engineers, Part C: Journal of Mechanical Engineering Science,
211, No.4, pp.273292.
[44] Li, Y., Lin, Z., Jiang, A., and Chen, G., 2004, "Experimental study of glassfiber mat
thermoplastic material impact properties and lightweight automobile body analysis",
Materials & Design, 25, No.7, pp.579585.
[45] Guo, Y., and Li, Y., 2007, "Quasistatic/dynamic response of SiO2–epoxy
nanocomposites", Materials Science and Engineering: A, 458, No.1, pp.330335.
[46] Omar, M.F., Md, A.H., Ahmad, Z.A., Mazuki, A.A.M, and Yokoyama, T., 2010,
"Dynamic properties of pultruded natural fibre reinforced composites using Split
Hopkinson Pressure Bar technique", Materials & Design, 31, No.9, pp.42094218.
83
CHAPTER 3 A STUDY OF THE DYNAMIC RESPONSE OF
THE NOVEL LAMINATED GLASS UNDER BLAST
LOADING
3.1. Introduction
In this chapter, a numerical model is proposed to characterize the dynamic response
of the fabricated laminated glass under blast loading. The validity of the proposed
numerical model has been proven by experimental results. Laminated glass’s failure
analysis is also performed in this chapter using the stress analysis approach.
3.2. Blast resistance testing
Field experiments were done at the Engineering Research and Development Center
(ERDC, US Army Corps of Engineers Lab, Vicksburg, Mississippi) using a Blast Load
Simulator (BLS). The thickness of the tested laminated glass was around 9.5 mm
(consisting of a 1/8 inch (3.2 mm) thick transparent composite interlayer laminated to two
1/8 inch (3.2 mm) thick tempered glass sheets). Sample gages were attached to the
laminated glass to record the pressure loading history and the midpoint deflection history
during the blast.
84
3.3 Blast resistance testing results
Both medium and high intensity blast loading tests were done at ERDC. The
pressuretime curve of the medium intensity blast is shown in Fig. 3.1. The key
parameters of the blast are obtained by curve fitting the initial pressure phase using
equation (1.1). The result of fitting is: peak overpressure Po =5.14 psi (35.4 kPa), constant
α=0.1011, and positive pressure duration time tp =11.3 ms.
Figure 3.1 Pressuretime curve of the medium intensity blast
Fig. 3.2 shows the midpoint deflection of the laminated glass under the medium
intensity blast shown in Fig. 3.1. It can be seen that the maximum deflection is about
0.415 inch (10.5 mm) and appears in the first deflection peak region.
85
Figure 3.2 Midpoint deflection of the laminated glass under the medium intensity blast
The pressuretime curve of the high intensity blast is shown in Fig. 3.3. The key
parameters of the blast are: peak overpressure Po=13.22 psi (91.1 kPa), constant =
0.2744, positive pressure duration time tp =15.4 ms.
Figure 3.3 Pressuretime curve of the high intensity blast
Fig. 3.4 shows the midpoint deflection of the laminated glass under the high
intensity blast shown in Fig. 3.3. The maximum deflection is around 0.99 inch (25.1 mm)
and also appears in the first deflection peak region.
First deflection peak region
86
Figure 3.4 Midpoint deflection of the laminated glass under the high intensity blast
Field experiments are important for understanding the dynamic response of the
laminated glass under blast loading. Besides field testing, modelbased analysis can also
be used to study the dynamic response of the laminated glass under blast loading. In this
study, a numerical model is proposed to characterize the dynamic response of the
fabricated laminated glass under blast loading.
3.4 Numerical modeling of the dynamic response of the fabricated
laminated glass under blast loading
According to Hamilton’s principle [1]
2
1
0 (3.1)
t
t
T W dt
where T is the kinetic energy of the laminated glass, is the strain energy of the
laminated glass and W is the work done by external load(s).
First deflection peak region
87
For the laminated glass, kinetic energy T can be calculated using the following
equation [2]
2
0 0
1(3.2)
2
a bw
T M dxdyt
where M is the unit area mass of the laminated glass and is equal to o o c c i ih h h . o ,
c and i are the density of the outer glass sheet, the composite interlayer and the inner
glass sheet, respectively. o i= =2600 kg/m
3 and c =1200 kg/m
3.
oh , ch , and hi are the
thickness of the outer glass sheet, the composite interlayer and the inner glass sheet,
respectively. In this study, o 3.2mmc ih h h . w is the transverse (thickness direction)
deflection of the laminated glass.
Strain energy can be calculated using the following equation [2]
1
= (3.3)2
x x y y xy xy
V
dxdydz
According to the classical plate theory [3], the strain components in the xy plane
(Fig. 3.5) can be expressed by the transverse deflection, w, as
2 2 2
2 2, , 2 (3.4)x y xy
w w wz z z
x y x y
88
z
y
x
ho
b
a
hc
hi
Blast pressure
Figure 3.5 Schematic diagram of the laminated glass
For the orthotropic composite interlayer, 2 21 1
c c cx x y
c c
E v E=
v v
,
21
c cy x
c
v E
v
21
cy
c
E
v
and xy c xyG , where Ec , Gc and vc are Young’s modulus, shear modulus and
Poisson’s ratio of the composite interlayer, respectively. It should be noted that the
mechanical properties of the glass fiberreinforced composite, such as Young’s modulus
and shear modulus, are influenced by strain rate [4]. However, in this analysis, since
strain rate was not measured in field testing, the strain rate effect is not considered. So Ec
, Gc and vc values used here are the values obtained from previous quasistatic mechanical
tests (Table 2.3). Substituting x , y and xy expressions into equation (3.3), the strain
energy of the composite interlayer is
89
2 2 2 2
1+ (3.5)
2 1 1 1 1
c c y x c c x y c y yc x xcomp c xy xy
c c c cV
E E EEG dxdydz
Integrating equation (3.5) through the transverse direction (thickness direction, z
direction) results in
2 23 32 2
2 2 2 2
23 32 2 2
0 0
2 2 2
12(1 ) 12(1 )13.6
2 2 4
12(1 ) 12
c c c c
a bc c
comp
c c c c c
c
E h E hw w
x ydxdy
E h G hw w w+
x y x y
where a is the length of the laminated glass, b is width of the laminated glass. In this
study, a = 0.89 m and b = 0.59 m.
Similarly, the strain energy of the outer and inner glass sheets is
2 2
3
g2
2 2 22 2 2 2 2
2 2 2 2
0 0
2 3 31= +
2 3(1 ) 4 2
2 2 1 (3.7)
g c g g c
glass
g
a b
g g
E h h h hh
w w w w wdxdy
x y x y x y
where hg is the thickness of one glass sheet (inner or outer layer glass sheet), Eg is
Young’s modulus of glass, vg is Poisson’s ratio of glass, In this study, tempered glass is
used, for which Eg = 68 GPa , vg = 0.2. Summing the strain energy of the composite
interlayer and glass sheets, the total strain energy of the laminated glass is
90
2 22
0 0
1(3.8)
2
a b
xx yy xx yy xyA w A w Bw w C w dxdy
2 2 33
2 2
2 2 33
2 2
2 2 33
2
2 3 3
4 23 1 12 1
2 3 3 22
4 23 1 12 1
2 3 3 42 1
4 2 123 1
g c g g c c cg
g c
g c g g c c c cg
g c
g c g g c c cg
g
E h h h h E hA= h +
E h h h h E hB= h +
E h h h h G hC= h +
where klw means a differentiation with respect to variable k and variable l.
For blast loading, the work done by external load is given by [2]
0 0
(3.9)
a b
W P t wdxdy
where P(t) is the instantaneous blast pressure and can be described by equation (1.1).
Substituting T , , W into equation (3.1), it can be rewritten as
2
0 0
= 0 (3.10)
t a b
xxxx yyyy xxyy
t
Mw w Aw Aw B C w w P t w dxdydt
where w means a secondorder derivative of w with respect to time. From equation
(3.10), the equation of motion of the laminated glass is obtained as
(3.11)xxxx yyyy xxyyMw A w w B C w P t
91
The laminated glass in this study is considered as simply supported. So the boundary
conditions are
0, 0, 0, ,
0, 0, 0, ,
xx
yy
w w at x a
w w at y b
The initial condition is
( , ,0) 0, ( , ,0) 0w x y w x y
In order to solve equation (3.11), an approximate function is chosen for w by
considering the simply supported boundary conditions [5, 6]
1 1
, , sin sin (3.12)m n
m x n yw x y t
a b
where is a unknown time dependent function. Here, for calculation convenience, m
and n are both simplified to 1. Substituting equation (3.12) into equation (3.11) and
applying Galerkin method, the equation of motion of the laminated glass is changed to
6 2 4 6 2 6 2 6 4
 /4 2
2 3 2 3 3
4 1 / e4 4 4 4 4
0
(3.13)
pt t
o p
A M b B b C b A ba b P t t a
b a b
Rearranging equation (3.13) and the following equation is obtained
92
6 2 6 2 6 42
6 /4
2 4 4
4 4 444 1 / e (3.14)
4
pt t
o p
B b C b A ba
Ab P t t
M b a
Equation (3.14) is a nonlinear ordinary differential equation and can be solved using
MATLAB. After obtaining function , the transverse deflection w can be calculated
using equation (3.12).
Besides the method shown above, equation (3.11) can also be solved by the
following procedures:
1) Equation (3.11) is converted to a secondorder ordinary differential equation us
ing double Fourier expansion.
2) The obtained ordinary differential equation is solved by Euler’s method.
The procedures for converting equation (3.11) to a secondorder ordinary
differential equation using double Fourier expansion are given in the Appendix A.
3.5 Comparison between numerical and experimental results
Fig. 3.6 shows the predicted maximum deflection state of the laminated glass under
the medium intensity blast loading. Fig. 3.7 shows the predicted maximum deflection
state of the laminated glass under the high intensity blast loading. In Fig. 3.6 and 3.7, the
laminated glass is simplified to a zerothickness plate. From Fig. 3.6 and 3.7, it can be
seen that the maximum deflection occurs at the midpoint. At the position close to the
93
edge of the laminated glass, the deflection decreases. This prediction correspnds fairly
well with the experimental results.
Figure 3.6 The maximum deflection state of the laminated
glass under the medium intensity blast loading
94
Figure 3.7 The maximum deflection state of the laminated
glass under the high intensity blast loading
From Fig. 3.2 and 3.4, it can be seen that the maximum deflection, which is an
important criterion for evaluating the blast resistance of the fabricated laminated glass,
occurs in the first deflection peak region. Therefore, the knowledge of the deflection
history in the first peak region is important and is simulated by the developed numerical
model. Fig. 3.8 shows the predicted midpoint deflection history in the first deflection
peak region. The predicted maximum deflection is 0.42 inch (10.6 mm) and the predicted
positive deflection duration time is 7.8 ms. The experimentally measured midpoint
95
deflection history (the circled region in Fig. 3.2) is also plotted in Fig. 3.8. The
experimentally measured maximum deflection value is 0.415 inch (10.5 mm) and the
meausred duration time is 8.3 ms. The discrepancy between the numerical result and the
experimental result may be caused by the neglect of the composite interlayer’s plastic
deformation and the strain rate effect on mechanical properties in the modeling. It can be
observed from Fig. 3.8 that for the medium intensity blast loading, the predicted result
matches well with the experimentally measured result.
Similarly, for the high intensity blast loading, the predicted midpoint deflection
history in the first deflection peak region is compared in Fig. 3.9 with the experimentally
measured result. The predicted maximum deflection is 1.03 inch (26.1 mm) and the
predicted positive deflection duration time is 8.1 ms. The experimentally measured
maximum deflection value is 0.99 inch (25.2 mm) and the measured duration time is 9.4
ms. Fig. 3.9 shows that for the high intensity blast loading, the predicted result also
matches fairly well with the experimentally measured result. Considering the good match
of the numerically predicted results and the experimentally measured results under
medium and high intensity blast loading, it can be concluded that the developed
numerical model is valid for predicting the dynamic reponse of the laminated glass under
both medium and high intensity blast loading.
96
Figure 3.8 Midpoint deflection of the laminated glass under the medium intensity blast loading in the first
deflection peak region
Figure 3.9 Midpoint deflection of the laminated glass under the high intensity blast loading in the first
deflection peak region
0 1 2 3 4 5 6 7 8 90
0.05
0.1
0.15
0.2
0.25
0.3
0.35
0.4
0.45
0.5
Time (ms)
Def
lect
ion
(in
ch)
Experimental result
Numberical result
0 1 2 3 4 5 6 7 8 9 100
0.2
0.4
0.6
0.8
1
Time (ms)
Def
lect
ion
(in
ch)
Experimental result
Numerical result
97
3.6 Laminated glass failure analysis
Based on the stressstrain relationship, the stresses of the laminated glass under blast
loading can be expressed as following equations
2
2
(3.15)1
1
avg
x x avg y
avg
avg
y avg x y
avg
xy avg xy
Ev
v
Ev
v
G
Substituting equation (3.4) into equation (3.15) results in
2 2
2 2 2
2 2
2 2 2
2
(3.16)1
1
2
avg
x avg
avg
avg
y avg
avg
xy avg
E z w wv
v x y
E z w wv
v x y
wG z
x y
where Eavg, vavg and Gavg are the average Young’s modulus, Poisson’s ratio and shear
modulus of the laminated glass, respectively. These parameters can be calculated using
the following equations [7]
98
2 1+
2 1+
g g c c g g
avg
g c g
g g c c g g
avg
g c g
g g g c c g g
avg
g g c g
E h E h E hE
h h h
v h v h v hv
h h h
E h v G h E hG
v h h h
After obtaining the values of the deflection w, the stresses of the laminated glass can be
calculated using equation (3.16). And then the principal stresses of the laminated glass
can be calculated. According to the literature [6], the maximum principal stress always
occurs at the midpoint of the laminated glass. So the midpoint maximum principal stress
history in the first and second deflection peak regions (the first positive deflection peak
region and the first negative deflection peak region) is calculated and compared with the
tensile strength of tempered glass to determine whether the laminated glass can survive
when subjected to blast loading. This criterion is proposed by Wei et al. and used in their
research [6]. The reason for studying the principal stress history in the first two deflection
peak regions only is that according to equation (3.16), stresses varies directly with the
deflection w. From Fig. 3.2 and 3.4, it can be observed that compared with the maximum
deflection (the first deflection peak), the deflection after the first two deflection peak
regions is small, which means corresponding stresses/principal stresses are small.
Therefore, in this study, the principal stress history after the first two deflection peak
regions is not discussed. When subjected to the medium intensity blast loading, the
midpoint maximum principal stress histories of the inner glass surface (pressure impact
99
surface) and the outer glass surface (pressure nonimpact surface) in the first two
deflection peak regions are calculated and plotted in Fig. 3.10.
Figure 3.10 Midpoint maximum principal stress history
under the medium intensity blast loading
Fig. 3.10 illustrates that for the inner surface, the maximum compression stress is
about 55 MPa and the maximum tensile stress is about 50 MPa; for the outer surface, the
maximum compression stress is about 31 MPa and the maximum tensile stress is about
85 MPa. The tensile strength of tempered glass is usually above 175 MPa (sometimes
above 200 MPa), and its compressive strength is much higher than its tensile strength [8
11]. Therefore, according to the stress analysis, the laminated glass will survive when
0 2 4 6 8 10 1260
40
20
0
20
40
60
80
100
Time (ms)
Str
ess
(MP
a)Inner surface
Outer surface
100
subjected to the medium intensity blast loading. This result has been proven by the
experimental result.
When subjected to the high intensity blast loading, the midpoint maximum principal
stress histories of the inner surface and the outer surface in the first two deflection peak
regions are shown in Fig. 3.11. From Fig. 3.11, it can be observed that the outer layer
glass first experiences its maximum tensile stress (around 200 MPa), which is close to but
not beyond the tensile strength of tempered glass. Then, the inner layer glass experiences
its maximum tensile stress (~95 MPa), which is lower than the tensile strength of
tempered glass. So, the laminated glass will survive after exposing to the high intensity
blast loading. This result corresponds with the experimentally observed result.
Figure 3.11 Midpoint maximum principal stress history
under the high intensity blast loading
0 2 4 6 8 10 12150
100
50
0
50
100
150
200
250
Time (ms)
Str
ess
(MP
a)
Inner surface
Outer surface
101
3.7 Summary
The dynamic response of the fabricated laminated glass under blast loading has been
investigated by field testing and modelbased analysis. The predicted response, in terms
of the midpoint deflection, agrees fairly well with the experimentally measured results
under medium and high intensity blast loading. Stress analysis and experimental results
both show that the fabricated laminated glass can survive under medium and high
intensity blast loading.
102
REFERENCES
[1] Pai, P.F., 2007, “Highly flexible structures: modeling, computation, and experimen
tation”, Reston, VA: American Institute of Aeronautics & Astronautics.
[2] Wei, J., 2004, "Dynamics and failure analysis of architectural glazing subjected to
blast loading", Rolla, MO: University of Missouri.
[3] Ugural, A.C., 1981, "Stresses in plates and shells", New York, NY: McGrawHill.
[4] Barre, S., Chotard, T., and Benzeggagh, M., 1996, "Comparative study of strain rate
effects on mechanical properties of glass fibrereinforced thermoset matrix composite",
Composites Part A: Applied Science and Manufacturing, 27, No.12, pp.11691181.
[5] Kazancı, Z., 2011, “Dynamic response of composite sandwich plates subjected to
timedependent pressure pulses”, International Journal of NonLinear Mechanics, 46,
No.5, pp.807817.
[6] Wei, J., and Dharani, L.R., 2006, "Response of laminated architectural glazing
subjected to blast loading", International Journal of Impact Engineering, 32, No.12,
pp.20322047.
[7] Vinson, J.R., 1999, "The Behavior of Sandwich Structures of Isotropic and Composite
Materials", Lancaster, PA: Technomic Publishing Company, Inc.
[8] Kalluri, R.S., 2007, "Failure of transparent polymer composite laminated glass
panels under impact loading", Columbia, MO: University of Missouri.
[9] Mencik, J., 1992, "Strength and fracture of glass and ceramics", New York, NY:
Elsevier.
[10] Veer, F., Zuidema, J., Bos, F., and Romein, T., 2005, "The strength and fracture
behaviour of annealed and tempered float glass", Proceedings of the 9th International
Conference on Architectural and Automotive Glass (GPD), pp.16.
[11] National Glass, "Glass Manufacture", http://www.nationalglass.com.au/catalogues/
NGP_Section_20.pdf.
103
CHAPTER 4 NONLINEAR DYNAMIC ANALYSIS OF THE
NOVEL LAMINATED GLASS UNDER BLAST LOADING
4.1 Introduction
In this chapter, the dynamic response of the fabricated laminated glass under a
medium intensity blast loading of peak pressure=5.14 psi (the same medium blast loading
as described in Chapter 3) is investigated using a new numerical model and a finite
element model. The numerical model analysis result and the finite element model
analysis result are compared with the experimentally measured result. Based on the new
numerical model, the blast resistance of the fabricated laminated glass is compared with
that of the same configuration laminated glass with PVB interlayer.
4.2 Numerical modeling and finite element modeling of the dynamic
response the fabricated laminated glass under blast loading
4.2.1 Numerical modeling
The schematic diagram of the laminated glass is shown in Fig. 4.1. It consists of a
1/8 inch (3.2 mm) thick transparent composite interlayer and two 1/8 inch (3.2 mm) thick
tempered glass sheets. The origin of the coordinate system of the laminated glass is set at
the corner of the midplane. The midplane (xy plane) is in the middle of the laminated
glass panel, with respect to the thickness direction.
104
z
y
x
ho
b
a
hc
hi
Blast Pressure
Figure 4.1 Schematic diagram of the laminated glass
(top and bottom layers are glass sheets, middle layer is the composite interlayer)
The straindisplacement relationship for a plate is [1, 2]
22
2
1= +  (4.1)
2x
u w wz
x x x
22
2
1= +  (4.2)
2y
v w wz
y y y
2
=2 = + + 2 (4.3)xy xy
u v w w wz
y x x y x y
where x , y and xy are strain components and u, v and w are displacement components
(in x, y and z directions, respectively).
The moments of a plate are [3]
105
2 2 2
    2 2 2
= = = (4.4)h h h
h h hx x y y xy xyM z dz M z dz M z dz
where h is the thickness of the plate. For the glass fiberreinforced orthotropic composite
interlayer, xc , yc and xyc are
2 21 1
c c cx y
c c
E v E
v v
,
2 21 1
c c cx y
c c
v E E
v v
, and c xyG ,
respectively. Ec , Gc and vc are Young’s modulus, shear modulus and Poisson’s ratio of
the composite interlayer, respectively. The values of Ec , Gc and vc are obtained from
Table 2.3. In this research, glass is considered as an isotropic material, xg , yg and xyg of
the glass sheets are 2 21 1
g g g
x y
g g
E v E
v v
,
2 21 1
g g g
x y
g g
E v E
v v
, and
2(1+ )
g
xy
g
E
v ,
respectively. gE and gv are Young’s modulus and Poisson’s ratio of glass sheets,
respectively. In this study, gE is 68 GPa and gv is 0.2.
First, substitute equations (4.1)(4.3) into xc , yc , xyc expressions, then substitute
the resultant xc , yc , xyc into equation (4.4) and integrate this equation through the
thickness direction. The moments of the composite interlayer ( , ,xc yc xycM M M ) can be
expressed as
106
3 2 2
2 22
3 2 2
2 22
3 2
= + (4.5)12 1
= +12 1
=6
c cxc c
c
c cyc c
c
c cxyc
E h w wM v
x y
E h w wM
x y
G h wM
x y
where ch is the thickness of the composite interlayer, in this study, hc = 3.2 mm.
Similarly, the moments of the glass sheets ( , ,xg yg xygM M M ) can be expressed as
2 2 2 23
2 22
2 2 2 23
2 22
2 2 23
3 3= + + +
2 43 1
3 3= + + + (4.6)
2 43 1
3 3= + +
2 43 1+
g g c g c
xg g g
g
g g c g c
yg g g
g
g g c g c
xyg g
g
E h h h h w wM h v
x y
E h h h h w wM h
x y
E h h h h wM h
x yv
where gh stands for the thickness of a glass sheet (inner or outer glass sheet), in this
study, gh = houter = hinner= 3.2 mm. It should be pointed out that for simplicity, only the
effect of the higherorder derivative component on moments is considered in this study.
The total moments of the laminated glass are
107
2 23 2 2 2 23
2 2 2 22 2
2 2 2 23
2 22
3 2 2
2 22 2
3 3= +  + + +
2 412 1 3 1
3 3  + + +
2 43 1
= + 12 1 3 1
g g c g cc cx c g g
c g
g g c g c
g g
g
gc cy c g
c g
E h h h hE h w w w wM v h v
x y x y
E h h h h w wh v
x y
EE h w wM h
x y
2 2 2 23
2 2
2 2 2 23
2 22
2 23 2 23
2 2
3
3 3+ + + (4.7)
2 4
3 3 + + +
2 43 1
3 3= + + +
6 2 43 1+
3 3+ + +
2 43 1+
g c g c
g
g g c g c
g g
g
g g c g cc cxy g
g
g g c g c
g
g
h h h h w w
x y
E h h h h w wh
x y
E h h h hG h w wM h
x y x yv
E h h h hh
v
2w
x y
According to references [3, 4], the equilibrium equation for the laminated glass is
2
2+ + + *= (4.8)
yxQQ w
q q mx y t
where
= + (4.9)
= 
yxxx
y xy
y
MMQ
x y
M MQ
y x
m is the unit area mass of the laminated glass and = g g c c g gm h h h , where g is the
density of the glass and is 2600 kg/m3.
c is the density of the composite interlayer and is
108
1200 kg/m3, q* is the resultant force caused by deflection and q is the external load acting
on the laminated glass which can be expressed using equation (1.1). Substituting equation
(4.9) into equation (4.8), and since xy yxM M , a new equilibrium equation is obtained
2 22 2
2 2 22 * (4.10)
y xyxM MM w
+  +q+q =mx y x y t
Substituting equation (4.7) and equation (1.1) into equation (4.10) results in
4 4 4 4 4 2
 /
4 2 2 2 2 4 2 2 2+ + + +2 + = 1 / e + *
(4.11)
pt t
o p
w w w w w wA B B A C m P t t q
x x y x y y x y t
where
33 2 2
2 2
2 3 3= + + +
2 412 1 3 1
gc cg g c g c
c g
EE hA h h h h h
v v
33 2 2
2 2
2 3 3+ + +
2 412 1 3 1
g gc c cg g c g c
c g
EE hB h h h h h
v v
33 2 2
2 3 3= + + +
6 2 43 1+
gc cg g c g c
g
EG hC h h h h h
v
Equation (4.11) can be rearranged to
4 4 4 2
 /
4 4 2 2 2+ + + = 1 / e (4.12)pt t
o p
w w w wD F m P t t q*
x y x y t
where
109
q* can be expressed as [3]
2 2 2 2 2 2
2 2 2 2* + 2 (4.13)
w w wq h
y x x y x y x y
where is called Airy’s stress function and is used to represent stresses: 2
x 2y
,
2
2yx
, 2
xyx y
, h is the thickness of the whole laminated glass and is equal to
hg+hc+hg. Substituting equation (4.13) into equation (4.12), equation (4.12) can be
rewritten as
 /+ + + = 1 / e + 2 (4.14)pt t
xxxx yyyy xxyy o p yy xx xx yy xy xyD w w Fw mw P t t h w w w
where ( )l means a differentiation with respect to variable l and w means a secondorder
derivative of w with respect to time. Equation (4.14) cannot be solved by itself. In order
to solve it, a St. Venant’s compatibility equation is introduced [3, 5], as listed below
2 22
2 22 (4.15)
y xyx
y x x y
33 2 2
2 2
3 33 2 2
2 2
2 3 3= + + +
2 412 1 3 1
4 3 3= + + + +
3 2 46 1 3 1
gc cg g c g c
c g
gc c c c cg g c g c
c g
EE hD h h h h h
v v
EE h v G hF h h h h h
v v
110
Rearranging equation (4.15) and substituting equations (4.1)(4.3) into equation (4.15),
results in equation (4.16)
2 (4.16)
22 22 2 2 2y xyx
2 2 2 2
w w w
y x x y x y x y
The strains shown in equation (4.16) can first be expressed in terms of stresses and then
in terms of Airy’s stress function. After substituting Airy’s function into equation
(4.16), a new compatibility equation is obtained as
2
+ + (4.17)yyyy xxxx xxyy xy xx yyN N P w w w
where
2
g c g
g g c c g g
g c g
c cg g c g g
c c c
h h hN
E h E h E h
h h hP
G EE h h E h
E v G
Equation (4.14) and (4.17) constitute a solvable system of nonlinear partial differential
equations, which are also the equations of motion for the fabricated laminated glass.
In this study, the laminated glass is considered as simply supported. So the boundary
conditions are
0, 0, at 0, (4.18)
0, 0, at 0,
xx
yy
w w x a
w w y b
111
The initial condition is
0, 0, at 0 (4.19)w w t
where a is the length of the laminated glass, which is 0.89 m and b is the width of the
laminated glass, which is 0.59 m.
Based on the boundary conditions, the following deflection mode shape is
assumed [6, 7],
1 1
, , sin sin (4.20)m n
x yw x y t t
a b
where (t) is an unknown function. For simplicity, equation (4.20) is approximated to its
first term. Substituting equation (4.20) into equation (4.17) results in
\
2 4
2 2
2 2+ + cos cos (4.21)
2yyyy xxxx xxyy
x yN N P
a b a b
The solution for this equation can be assumed as [6]
2
1 2
1 2 2cos cos (4.22)
x yf f
N a b
Substituting equation (4.22) into the left part of equation (4.21) results in
4 42
1 24 4
16 2 16 2+ + cos cos (4.23)yyyy xxxx xxyy
x yN N P f f
a a b b
112
Therefore, equation (4.21) can be rewritten as
4 42
1 24 4
16 2 16 2cos cos
x yf f
a a b b
=
2 4
2 2
2 2cos cos (4.24)
2
x y
a b a b
From equation (4.24), it can be inferred that 2
1 2=
32
af
b and
2
2 2=
32
bf
a, so the solution for
equation (4.24) is obtained. Introducing the solution and equation (4.20) into equation
(4.14) and applying Galerkin method to equation (4.14), the nonlinear partial differential
equation (4.14) is changed to a nonlinear ordinary differential equation with respect to
time
4 4 2 2 4 4 3 4 4
2 3 3 3 3
41 0 (4.25)
4 4 64
p
t
to
p
Da Fa b Db h a babPabm te
t a b a b N
where is the secondorder derivative of with respect to time. Equation (4.25) can be
solved using MATLAB. After obtaining the function , the transverse deflection w can
be calculated using equation (4.20).
Besides the transverse deflection, the principal stresses of the laminated glass under
blast loading can also be obtained through this model by the following procedures:
1) After obtaining the transverse deflection, since the straindisplacement
relationships are known from equations (4.1)(4.3), so the strains of the laminated glass
can be calculated (ignore the displacements in x and y directions).
113
2) According to the stressstrain relationships of the laminated glass [6, 8], the
bending stresses of the laminated glass can be calculated. The membrane stresses of the
laminated glass can be calculated using Airy’s stress function [9].
3) By adding the bending and membrane stresses together, the total stresses of the
laminated glass are obtained
22 2 2 2
2 2 2 2
22 2 2 2
2 2 2 2
1 1+ (4.26)
1 2 2
1 1
1 2 2
avg
x avg
avg
avg
y avg
avg
xy avg
E w w w wz v z
v x x y y y
E w w w wv z z
v x x y y x
w wG
x
2 2
2w
zy x y x y
where Eavg, vavg and Gavg are the average Young’s modulus, Poisson’s ratio and shear
modulus of the laminated glass, respectively.
4) The principal stresses of the laminated glass can be calculated based on the total
stresses.
4.2.2 Finite element modeling
In this research, the dynamic response of the laminated glass is also studied using
the finite element software ANSYS. The laminated glass is discretized by the fournode
shell element SHELL181. 280 elements are used for discretization.
114
SHELL181 element is suitable for analyzing thin to moderately shell structures,
including composite shells and sandwich constructions [10, 11].
The following figure shows the geometry of this element.
J
KL
Z
X
Y
I
Figure 4.2 SHELL181 geometry [10]
(I, J, K and L are nodes)
The shell section commands of the SHELL181 element allow for sandwich structure
definition. Options are available for specifying the thickness, material, orientation and
number of integration points through the thickness of sandwich structure layers (Fig. 4.3).
Figure 4.3 Shell section page
115
Materials properties obtained from mechanical tests and blast constants (Po, and
tp) obtained from blast curve fitting are used as inputs in the finite element modeling.
4.3 Results and discussions
4.3.1 Midpoint deflection
The dynamic response, in terms of the midpoint deflection, of the laminated glass
under the medium intensity blast loading is predicted using the new numerical mode and
the finite element model, respectively. The experimentally measured result is compared
with the numerical modeling result and the finite element modeling result (Fig. 4.4).
From this figure, it can be seen that both the numerical modeling result and the finite
element modeling result match well with the experimentally measured result, especially
in predicting the peak deflection. However, the discrepancy is more apparent during the
unloading phase. The discrepancy between the experimentally measured result and the
analytically predicted results (finite element modeling result and numerically modeling
result) may be caused by the neglect of the composite interlayer’s plastic deformation and
the strain rate effect on mechanical properties in the modeling.
116
Figure 4.4 Midpoint deflection comparison
Since both the numerical model and the finite element model can describe the
dynamic response of the laminated glass, both models are used to study the midpoint
maximum principal stress history of the laminated glass as it is an important criterion for
determining whether a laminated glass fails when subjected to a blast loading [6].
4.3.2 Midpoint maximum principal stress history
Fig. 4.5 and Fig. 4.6 demonstrate the midpoint maximum principal stress history of
the inner glass surface (pressure impact surface) and outer glass surface (pressure non
0 0.001 0.002 0.003 0.004 0.005 0.006 0.007 0.008 0.009 0.01 0.0111
0.8
0.6
0.4
0.2
0
0.2
0.4
0.6
0.8
1
Time (s)
Def
lect
ion
(in
ch)
Finite element modeling result
Numerical modeling result
Experimental result
117
impact surface), respectively. The blue line in these figures represents the finite element
model calculated result and the red line represents the numerical model calculated result.
From Fig. 4.5, it can be observed that for the inner glass surface, the maximum
compression stresses calculated using the finite element model and the new numerical
model are close and approximately 45 MPa. But the calculated maximum tensile stresses
are a little different. The result calculated using the finite element model is around 60
MPa and the result calculated using the numerical model is around 45 MPa. From Fig.
4.6, it can be observed that for the outer glass surface, the maximum tensile stress
calculated using the finite element model is around 105 MPa and the tensile stress
calculated using the numerical model is around 95 MPa. The maximum compression
stress calculated using the finite element method is around 45 MPa and the compression
stress calculated using the numerical model is around 25 MPa. On the whole, the
numerical modeling results match with the basic variation of the finite element modeling
results. However, there is a variation of about 1020% in the prediction of the peak
principle stress values between the two methods. Since the tensile strength of tempered
glass is usually higher than 175 MPa and its compressive strength is much higher than its
tensile strength [1215], the fabricated laminated glass is expected to survive when
subjected to the medium intensity blast loading. This has been proven by the field testing
result.
118
Figure 4.5 Midpoint maximum principal stress history of the inner glass surface
Figure 4.6 Midpoint maximum principal stress history of the outer glass surface
0 0.005 0.01 0.015150
100
50
0
50
100
150
Time (s)
Str
ess
(MP
a)
Finite element modeling result
Numerical modeling result
0 0.005 0.01 0.015100
50
0
50
100
150
200
Time (s)
Str
ess
(MP
a)
Finite element modeling result
Numerical modeling result
119
The midpoint deflection and maximum principle stresses of the laminated glass with
PVB interlayer can also be predicted using the new numerical model and the finite
element model by setting the interlayer properties to the properties of PVB. Young’s
modulus and Poisson’s ratio of PVB are 100 MPa and 0.448, respectively [16]. When
subjected to the medium intensity blast loading used in this chapter, the midpoint
deflections of the laminated glass with the composite interlayer and the laminated glass
with PVB interlayer are plotted in Fig. 4.7 (results obtained from the new numerical
model. Results obtained from the finite element model are similar, so not shown here).
From Fig. 4.7, it can be observed that compared with the same configuration laminated
glass with the composite interlayer, the maximum deflection of the laminated glass with
PVB interlayer is larger. The midpoint maximum principal stresses of the inner surface
and the outer surface are plotted in Fig. 4.8 and Fig. 4.9, respectively. These figures
demonstrate that the midpoint maximum principal stresses (inner surface and outer
surface) of the laminated glass with PVB interlayer are larger than those of the laminated
glass with the composite interlayer. These results means the laminated glass with PVB
interlayer is more likely to fail when both laminated glasses subjected to the same
intensity blast loading.
120
Figure 4.7 Comparison of midpoint deflections under the medium intensity blast loading
0 0.002 0.004 0.006 0.008 0.01 0.0110.2
0.1
0
0.1
0.2
0.3
0.4
0.5
Time(s)
Def
lect
ion
(in
ch)
Laminated glass with the composite interlayer
Laminated glass with PVB interlayer
121
Figure 4.8 Comparison of midpoint maximum principal stresses (inner surface)
0 0.005 0.01 0.015100
80
60
40
20
0
20
40
60
80
100
Time (s)
Str
ess
(MP
a)
Laminated glass with the composite interlayer
Laminated glass with PVB interlayer
122
Figure 4.9 Comparison of midpoint maximum principal stresses (outer surface)
4.4 Summary
The dynamic response of the fabricated laminated glass under a medium intensity
blast loading is studied using a new numerical model and a finite element model. The
predicted result, either using the numerical model or the finite element model, agrees well
with experimentally measured result.
Stress analysis shows the fabricated laminated glass can survive when subjected to
the medium intensity blast loading. This has been proven by the field experimental result.
Dynamic response analysis and stress analysis both show that under the same intensity
0 0.005 0.01 0.01560
40
20
0
20
40
60
80
100
120
140
Time (s)
Str
ess
(MP
a)
Laminated glass with the composite interlayer
Laminated glass with PVB interlayer
123
blast, the laminated glass with fiberreinforced composite interlayer performs better than
the same configuration laminated glass with PVB interlayer. In other words, to reach the
same protection effect, the laminated glass with the composite interlayer can be
fabricated thinner and lighter.
124
REFERENCES
[1] Kazancı Z., 2011, "Dynamic response of composite sandwich plates subjected to time
dependent pressure pulses", International Journal of NonLinear Mechanics, 46, No.5,
pp.807817.
[2] Kazanci, Z., and Mecitoglu, Z., 2006, "Nonlinear damped vibrations of a laminated
composite plate subjected to blast load", AIAA Journal, 44, No.9, pp.20022008.
[3] Nishawala, V., 2011, "A study of large deflection of beams and plates", New
Brunswich, NJ: Rutgers University.
[4] Riber, H.J., 1997, "Nonlinear analytical solutions for laterally loaded sandwich
plates", Composite Structures, 39, No.1, pp.6383.
[5] Ugural, A.C., 1981, "Stresses in plates and shells", New York, NY: McGrawHill.
[6] Wei, J., and Dharani, L.R., 2006, "Response of laminated architectural glazing
subjected to blast loading", International Journal of Impact Engineering, 32, No.12,
pp.20322047.
[7] Teng, T.L., Liang, C.C., and Liao, C.C., 1996, "Transient dynamic largedeflection
analysis of panel structure under blast loading", JSME International Journal Series A,
Mechanics and Material Engineering, 39, No.4, pp.591597.
[8] Vinson, J.R., 1999, "The behavior of sandwich structures of isotropic and composite
materials", Lancaster, PA: Technomic Publishing Company.
[9] Brubak, L., Hellesland, J., Steen, E., and Byklum, E., 2004, "Approximate buckling
strength analysis of plates with arbitrarily oriented stiffeners", Proceedings of the 17th
Nordic Seminar on Computational Mechanics (NSCM17), pp.5053.
[10] ANSYS, "ANSYS Help", Canonsburg, PA: ANSYS.
[11] ANSYS, "SHELL181", http://mostreal.sk/html/elem_55/chapter4/ES4181.htm.
[12] Kalluri, R.S., 2007, "Failure of transparent polymer composite laminated glass
panels under impact loading", Columbia, MO: University of Missouri.
[13] Mencik, J., 1992, "Strength and fracture of glass and ceramics", New York, NY:
Elsevier.
[14] Veer, F., Zuidema, J., Bos, F., and Romein, T., 2005, "The strength and fracture
behaviour of annealed and tempered float glass", Proceedings of the 9th International
Conference on Architectural and Automotive Glass (GPD), pp.16.
125
[15] National Glass, "Glass Manufacture", http://www.nationalglass.com.au/catalogues/
NGP_Section_20.pdf.
[16] Bennison, S.J., Qin, M.H., and Davies, P.S., 2008, "Highperformance laminated
glass for structurally efficient glazing", Innovative LightWeight Structures and
Sustainable Facades, pp.112.
126
CHAPTER 5 CONCLUSIONS AND FUTURE WORK
In this research, a transparent glass fiberreinforced polyester composite has been
developed. The transparent glass fiberreinforced composite was fabricated by matching
the refractive index of the polyester matrix with that of glass fibers. The light
transmittance of the composite varies with light wavelength and can reach up to a
maximum of 74.5% for a wavelength of 600 nm. Different tests have been used to
determine the properties of the composite. Tensile test was used to find Young’s
modulus, Poisson’s ratio and Shear modulus. Jintegral test was used to find the fracture
toughness.
The transparent composite developed was used to fabricate a novel blastresistant
laminated glass. The dynamic response of the fabricated laminated glass under blast
loading was tested using a Blast Load Simulator. The dynamic response is also
analytically investigated using modelbased method and finite element method. The
modelbased analysis is conducted based on two numerical models. The equations of
motion of two models are partial differential equations. In order to solve these equations,
Galerkin method is used to change these equations to nonlinear ordinary differential
equations and these nonlinear ordinary differential equations are solved using Runge
Kutta method in MATLAB. After obtaining the solutions of these equations, the dynamic
response of the fabricated laminated glass is characterized. The finite element analysis is
performed using the commercial finite element software ANSYS. The analytically
calculated results (results obtained from the modelbased analysis and the finite element
127
analysis) are compared with the experimentally measured results. Comparison results
show that analytically calculated results match well with the experimentally measured
results, which proves the validity of the developed numerical models and the finite
element model. Stress analysis of the fabricated laminated glass shows that a 3/8 inch
thick laminated glass panel can survive when subjected to both medium and high
intensity blast loading and compared with the same configuration laminated glass with
PVB interlayer, it has better blast resistance.
To sum up, a novel laminated glass has been fabricated. The dynamic response of
the fabricated laminated glass under blast loading has been investigated. Though a lot of
work has been devoted to the fabrication and study of this laminated glass, this laminated
glass could be further improved through some modifications and further study as
suggested below:
1) More transparent composite interlayer. Though the developed glass fiber
reinforced composite interlayer has good transparency, the transparency of the composite
interlayer can be further increased, like increasing to more than 80% at any wavelength in
the visible light region. One possible way to further increase the transparency of the
composite interlayer is to find new chemical additives to further reduce the refractive
index difference between glass fibers and the polyester matrix.
2) Better laminated glass fabrication method. Presently, the laminated glass panels
are fabricated using the hand layup technique. This technique is the simplest one to
fabricate the laminated glass. This technique requires minimal investment in molds but is
not suitable for mass production. Also this technique may introduce air bubbles at the
128
interfaces between the composite interlayer and glass sheets during lamination, which can
reduce the transparency of the laminated glass. Therefore, a better technique is needed for
the potential mass production.
3) More precise numerical model. The numerical models developed are good for
predicting the dynamic response of the fabricated laminated glass under blast loading.
But there are still gaps between the experimentally measured results and the predicted
results. The discrepancy may be caused by the neglect of the composite interlayer’s
plastic deformation and the strain rate effect on mechanical properties in the modeling. If
the plastic deformation and the strain rate effect are considered in the modeling, a more
precise numerical model can be established and thereby, the dynamic response of the
laminated glass under blast loading can be predicted more precisely.
129
APPENDIX A
The procedures for converting equation (3.11) to a secondorder ordinary
differential equation are shown below
 /
(A.1)
1 / e p
xxxx yyyy xxyy
t t
o p
Mw A w w B C w P t
P t P t t
where M is the unit area mass of the laminated glass, A, B and C are constants, Po is the
peak pressure of a blast loading, is a constant and tp is the positive pressure duration
time of the blast. By using double Fourier expansion, Po can be expanded as
1 1
sin sinmn
m n
m x n yP
a b
, where mnP is an unknown function, m and n are positive
integers, a and b are the length and width of the laminated glass, respectively [1].
Similarly, w, which is the thickness direction displacement component, can be expanded
as 1 1
sin sinmn
m n
m x n yW t
a b
, where mnW t is an unknown time function.
Therefore,
4
1 1
sin sinxxxx mn
m n
m m x n yw W t
a a b
4
1 1
sin sinyyyy mn
m n
n m x n yw W t
b a b
2 2
1 1
sin sinxxyy mn
m n
m n m x n yw = W t
a b a b
''
1 1
sin sinmn
m n
m x n yw W t
a b
130
where ''
mnW t is the secondorder derivative of mnW t in respect of time t.
Substitute , , , ,o xxxx yyyy xxyyP w w w w into equation (A.1), equation (A.1) can be rewritten
as
4
''
1 1 1 1
4
1 1
2
sin sin sin sin
sin sin (A.2)
mn mn
m n m n
mn
m n
m x n y m m x n yM W t A W t
a b a a b
n m x n yA W t
b a b
m nB C
a b
2
1 1
1 1
sin sin
sin sin 1 p
mn
m n
tt
mn
m n p
m x n yW t
a b
m x n y tP e
a b t
Simplify equation (A.2) and get
4 2 2 4
+ + + = 1 (A.3)p
αtt''
mn mn mn
p
mπ mπ nπ nπ tA B+C A W t MW t P  e
a a b b t
Let 4 2 2 4
= + +mπ mπ nπ nπ
J A B+C Aa a b b
Equation (A.3) can be rewritten as,

''+ = 1 (A.4)p
tt
mn mn mn
p
tJW t MW t P e
t
131
In equation (A.4), mnP is the only unknown coefficient. If the value of
mnP can be
obtained, equation (A.4) can be solved using Euler’s method. The unknown coefficient
mnP can be obtained through following procedures proposed by Timoshenko [1, 2]:
Since,
1 1
sin sino mn
m n
m x n yP P
a b
Multiply each side of above equation by 0
0sin
b n y
b
where n0 is an arbitrary integer,
obtains
0 0
0 01 1
sin sin sin sin (A.5)b b
o mn
m n
n y n ym x n yP dy P dy
b a b b
According to identity principle [1],
0
0
00
0 if
sin sinif =
2
bn n
n y n ydy b
b b n n
So,
0
01
sin sin2
b
n
n y n y bdy
b b
Equation (A.5) can be rewritten as
0
01
sin sin (A.6)2
b
o mn
m
n y b m xP dy P
b a
132
Similarly, multiply equation (A.6) by 0
0sin
a m x
a
, where m0 is an arbitrary integer
number, obtains
0 0 0
0 0 01
sin sin sin sin (A.7)2
a b a
o mn
m
m x n y m xb m xP dx dy P dx
a b a a
Still according to the identity principle,
0
0
00
0 if
sin sinif =
2
am m
m x m xdx a
a a m m
So,
0 0
0 0sin sin (A.8)
4
a b
o mn
m x n y abP dx dy P
a b
mnP can be expressed as
0 0
4sin sin (A.9)
a b
mn o
m x n yP dx P dy
ab a b
Integrate equation (A.9) and get the value of mnP
133
0 0 0 0
0
44sin sin sin sin
4 4sin cos sin
a b a bo
mn o
ba
o o
0
Pm x n y m x b n y n yP dx P dy dx d
ab a b ab a n b b
P Pm x b n y b m xdx
ab a n b ab n a
0
0 00
cos 1
8 8 8 16sin sin cos( )
a
aa a
o o o o
2 2
n
P b P b P Pm x a m x m x m xdx d
abn a abn m a a nm a nm
when m, n=1, 3, 5....
Substitute the value of mnP into equation (A.4),

'' 16+ = 1 (A.10)p
tto
mn mn 2
p
P tJW t MW t e
nm t
As mentioned previously, equation (A.10) can be solved using Euler’s method.
After getting the values of time function mnW t , w, the thickness direction displacement
component, can be calculated using the equation 1 1
sin sinmn
m n
m x n yW t
a b
.
134
REFERENCES
[1] Auburn University, "Plates Subjected to Transverse Loads".
[2] Timoshenko, S., Woinowsky, K.S., and Woinowsky, S., 1959, "Theory of plates and
shells", New York, NY: McGrawHill.
135
VITA
Hua Zhu was born on November 9th, 1982 in Yantai, Shandong, China. He got his
Bachelor’s degree in Polymer Science and Engineering from Yantai University (Yantai,
China) in 2005. After that, he studied at Nanjing University of Technology (Nanjing,
China), where he graduated with his Master’s degree in Materials Science in 2008. At the
same year, he came to the United States and studied at University of Massachusetts
Lowell for one year. Then he transferred to University of MissouriColumbia and started
his Ph.D. study under the supervision of Dr. Sanjeev K. Khanna. He is married to Tianyi
Qiu, who is studying physiology in Physiology and Pharmacology Department at
University of MissouriColumbia.